# VLFV - Eötvös Loránd Universitymetal.elte.hu/~ispanovity/kornel/zaiser_2006.pdf · Plasticity,...

Embed Size (px)

### Transcript of VLFV - Eötvös Loránd Universitymetal.elte.hu/~ispanovity/kornel/zaiser_2006.pdf · Plasticity,...

PLEASE SCROLL DOWN FOR ARTICLE

7KLV�DUWLFOH�ZDV�GRZQORDGHG�E\��>.DUOVUXKHU�,QVW�IXU�7HFKQRORJLH�.LW@2Q����'HFHPEHU�����$FFHVV�GHWDLOV��$FFHVV�'HWDLOV��>VXEVFULSWLRQ�QXPEHU����������@3XEOLVKHU�7D\ORU��)UDQFLV,QIRUPD�/WG�5HJLVWHUHG�LQ�(QJODQG�DQG�:DOHV�5HJLVWHUHG�1XPEHU����������5HJLVWHUHG�RIILFH��0RUWLPHU�+RXVH��������0RUWLPHU�6WUHHW��/RQGRQ�:�7��-+��8.

$GYDQFHV�LQ�3K\VLFV3XEOLFDWLRQ�GHWDLOV��LQFOXGLQJ�LQVWUXFWLRQV�IRU�DXWKRUV�DQG�VXEVFULSWLRQ�LQIRUPDWLRQ�KWWS���ZZZ�LQIRUPDZRUOG�FRP�VPSS�WLWOHaFRQWHQW W���������

6FDOH�LQYDULDQFH�LQ�SODVWLF�IORZ�RI�FU\VWDOOLQH�VROLGV0LFKDHO�=DLVHUDD�7KH�8QLYHUVLW\�RI�(GLQEXUJK��,QVWLWXWH�IRU�0DWHULDOV�DQG�3URFHVVHV��(GLQEXUJK�(+���-/��8.

7R�FLWH�WKLV�$UWLFOH�=DLVHU��0LFKDHO�������6FDOH�LQYDULDQFH�LQ�SODVWLF�IORZ�RI�FU\VWDOOLQH�VROLGV��$GYDQFHV�LQ�3K\VLFV������������٢����7R�OLQN�WR�WKLV�$UWLFOH��'2,���������������������������85/��KWWS���G[�GRL�RUJ��������������������������

Full terms and conditions of use: http://www.informaworld.com/terms-and-conditions-of-access.pdf

This article may be used for research, teaching and private study purposes. Any substantial orsystematic reproduction, re-distribution, re-selling, loan or sub-licensing, systematic supply ordistribution in any form to anyone is expressly forbidden.

The publisher does not give any warranty express or implied or make any representation that the contentswill be complete or accurate or up to date. The accuracy of any instructions, formulae and drug dosesshould be independently verified with primary sources. The publisher shall not be liable for any loss,actions, claims, proceedings, demand or costs or damages whatsoever or howsoever caused arising directlyor indirectly in connection with or arising out of the use of this material.

Advances in Physics,Vol. 55, Nos. 1–2, January–April 2006, 185–245

Scale invariance in plastic flow of crystalline solids

MICHAEL ZAISER*

The University of Edinburgh, Institute for Materials and Processes,The King’s Buildings, Sanderson Building, Edinburgh EH9 3JL, UK

(Received 31 October 2005; in final form 17 January 2006)

From the traditional viewpoint of continuum plasticity, plastic deformation ofcrystalline solids is, at least in the absence of so-called plastic instabilities,envisaged as a smooth and quasi-laminar flow process. Recent theoretical andexperimental investigations, however, demonstrate that crystal plasticity ischaracterized by large intrinsic spatio-temporal fluctuations with scale-invariantcharacteristics: In time, deformation proceeds through intermittent bursts withpower-law size distributions; in space, deformation patterns and deformation-induced surface morphology are characterized by long-range correlations,self-similarity and/or self-a!ne roughness. We discuss this scale-invariantbehaviour in terms of robust scaling associated with a non-equilibrium criticalpoint (‘yielding transition’).

Contents page1. Introduction 186

1.1. Continuum mechanics of crystal plasticity 1871.2. Crystal plasticity on the dislocation level: yield stress and depinning transition 191

2. Experimental investigation of fluctuation phenomena in plastic flow 1972.1. Acoustic emission measurements 197

2.1.1. Experimental methodology 1972.1.2. Acoustic emission in single- and polycrystals of ice 1982.1.3. Acoustic emission in metals and alloys 201

2.2. Deformation-induced surface patterns 2022.2.1. Slip-line patterns 2022.2.2. Slip-line kinematography 2032.2.3. Surface roughening in single- and polycrystals 205

2.3. Deformation of micron-size samples 2093. Theoretical approaches 212

3.1. Dislocation dynamics 2133.1.1. Simulation methods 2133.1.2. Relaxation and creep of two-dimensional dislocation systems 2183.1.3. Stepwise deformation curves and critical behaviour at yield 220

3.2. Models of microstrain evolution 2243.2.1. Constitutive equations 2243.2.2. Avalanche dynamics and surface morphology evolution 227

3.3. Phase-field models 233

*Email: [email protected]

Advances in PhysicsISSN 0001–8732 print/ISSN 1460–6976 online # 2006 Taylor & Francis

http://www.tandf.co.uk/journalsDOI: 10.1080/00018730600583514

Downloaded By: [Karlsruher Inst fur Technologie Kit] At: 14:00 9 December 2010

4. Discussion and conclusions 2364.1. Why has it not been seen before? 2374.2. Open questions, doubts and prospects 240

Acknowledgements 243References 243

1. Introduction

According to the traditional paradigm implicit in continuum models of plasticity,crystalline solids are considered as homogeneous continua which, in the absence ofso-called plastic instabilities, deform under homogeneous loads in a smooth andspatially homogeneous manner. Fluctuations are supposed to average out abovethe scale of a ‘representative volume element’ which is assumed to be small incomparison with the dimensions of the deforming body. Spatio-temporal deforma-tion patterning may, according to this viewpoint, occur only if the deformationprocess is macroscopically unstable due to some mechanism which produces strainor strain rate softening. Macroscopic plastic instabilities of this type give rise tospatio-temporal patterns in the form of stationary or travelling solitary waves(see, e.g. the Scripta Materialia Viewpoint set edited by Kubin, Estrin andAifantis [1]) and to oscillatory and/or chaotic deformation modes (see the reviewsby Zaiser and Hahner [2] and by Kubin, Fressengeas and Ananthakrishna [3]). Thesephenomena have been studied in some detail in conjunction with the general enthu-siasm for nonlinear phenomena in the 1980s and early 1990s, but were generallylooked upon as representing some kind of scientifically interesting, but non-genericbehaviour, out of the ordinary and of limited practical importance.

The paradigm of plastic flow as a smooth process has a counterpart in the workof materials scientists investigating the micromechanisms of crystal plasticity, viz.,the motion of the line defects (dislocations) which in a crystal lattice carry discrete‘quanta’ of slip. Due to the discreteness of dislocations, plastic flow on the‘microscopic’ scale of individual dislocations is necessarily inhomogeneous inspace and often, due to the presence of localized obstacles, intermittent in time.However, in line with the continuum paradigm, the prevailing viewpoint was thatmicroscopic deformation localization and intermittency are irrelevant as soon asmultiple defects are involved, since the incoherent superposition of individual defectmotions would result in a smooth and approximately homogeneous flow. It is anassumption implicit in much of the materials science work on plasticity that lack ofcoherency in the individual defect processes leads to deformation behaviour that isstatistically homogenous on the mesoscopic scale of multiple defects. This assump-tion is also convenient from a modelling viewpoint, since it allows us to draw directconclusions from the properties of individual defects, or from their pair interactions,on the macroscopic material behaviour.

Recently, however, the traditional paradigm of ‘stable’ plastic deformation as asmooth and steady flow process has been challenged both from an experimental andfrom a theoretical point of view (see, e.g. [4–8]). From these works, a quite di"erentpicture of plastic flow emerges: Instead of the incoherent motion of individual

186 M. Zaiser

Downloaded By: [Karlsruher Inst fur Technologie Kit] At: 14:00 9 December 2010

defects, one finds coherent bursts of activity with long-range correlations both inspace and in time. Such correlated bursts are detected in situations where thetraditional paradigm leads one to expect to find a smooth and homogeneous flow.The properties of these bursts also di"er from those commonly associated withplastic instabilities: Instead of coherent spatio-temporal oscillations one findsrandom bursts with scale-free size distributions, instead of plastic wave propagationone sees long-range correlated deformation patterns with self-similar or self-a!necharacteristics, and instead of the emergence of characteristic internal length andtime scales one observes scale-free behaviour in space and in time. In short, thepicture is that of critical phenomena commonly associated with phase transitions,rather than that of coherent nonlinear behaviour.

In the present review we summarize experimental and theoretical work on the(almost) scale-free fluctuation phenomena that can be observed in deformingcrystals. In the rest of the introduction, we give a brief summary of continuummechanics approaches towards crystal plasticity, which mainly serves to introducerelevant terminology used by the continuum mechanics community. We also discussthe yielding of a crystal on the dislocation level (dislocation depinning); in thiscontext we present the reader with a set of phenomena that have been studied bystatistical physicists in the general context of the dynamics of elastic manifolds inrandom media, and which will recur in one form or another throughout the subse-quent chapters. In our section on experimental observations, we discuss in somedetail acoustic emission (AE) measurements which are possibly the most usefulavailable tool for monitoring the temporal dynamics of plastic flow in situ. Wealso discuss the surface-based in situ and post mortem investigation of deformationpatterns based on the study of traces of dislocation motion (slip lines), and theanalysis of deformation-induced changes in the overall surface morphology (surfaceroughening). We then discuss the theoretical modelling of flow phenomena in termsof the dynamics of interacting dislocations, in terms of phenomenological continuummodels describing the evolution of plastic strain above the dislocation scale, andin terms of phase-field models which in a sense are in between the former twoapproaches. We demonstrate that these approaches result in a consistent pictureof the main characteristics of the ‘yielding transition’ which can qualitatively orsemi-quantitatively account for many of the pertinent experimental observations,though several open questions remain. It is important to note that the present reviewdoes not account for all types of scale-free behaviour in plastically deformingcrystals: We exclude the entire realm of plastic instabilities, in particular thescale-free statistics of load drops associated with the so-called PLC e"ect [3]. Wealso exclude from our discussion the scale-free defect microstructures which emergeduring deformation of crystals in certain high-symmetry orientations [9, 10] but areabsent under other deformation conditions and may, hence, represent a non-genericfeature.

1.1. Continuum mechanics of crystal plasticity

We first discuss the conventional continuum mechanics approach towards crystalplasticity. Besides illustrating the pertinent concepts and mindset, this serves to

Scale invariance in plastic flow of crystalline solids 187

Downloaded By: [Karlsruher Inst fur Technologie Kit] At: 14:00 9 December 2010

introduce a set of notations that will structure our discussion throughout thepresent review.

Plasticity, reversible and irreversible deformation Plastic deformation can be looselydefined as any deformation of a solid body that persists after the driving forceapplied to the deforming body is removed. Of necessity this implies changes inneighbourhood relations between atoms. In general, plasticity is isochoric, i.e. thevolume of the deforming body is not changed. Plastic deformation is always anirreversible process in the thermodynamic sense, but conversely not everythermodynamically irreversible deformation process is plastic: viscoelastic behaviourdissipates energy, even though the initial shape of the body is restored once the forcesare removed (no plasticity), viscous flow of a liquid entails both dissipation and anirreversible change in shape, but the deforming body is not solid (i.e. it does notpossess a finite yield stress, cf. below). In a plastically deforming solid, we may splitthe total strain tensor ! into an elastic and a plastic part. Throughout this paperwe adopt a small-strain formulation, such that an additive decomposition is feasible:

! ! !el " !pl: #1$

In a linearly elastic material the elastic strain is related to the stress D via !el ! C%1Dwhere C is Hooke’s tensor of elastic moduli. If the stress is removed, the plastic strain!pl remains.

Crystal plasticity, crystallographic slip Plasticity of crystalline solids is constrainedby the fact that any occurring atomic rearrangements must preserve the crystallattice structure. (We exclude from our discussion transformation-induced plasticity,where deformation is due to a stress-driven transition between crystalline phaseswith di!erent lattice structures.) This implies that deformation must occur byshear of adjacent lattice planes such that the displacement of one plane againstthe other is by a lattice vector contained in the plane. A set of crystallographic planescharacterized by their common unit normal vector n, and a corresponding latticevector b (also called the Burgers vector), constitute a slip system. In most crystals,deformation is observed on a small number of slip systems only, often correspondingto the most densely packed planes and lattice directions (e.g. deformation of face-centred cubic crystals occurs usually on slip systems of the type f111g[110]).

The plastic strain tensor !pl can be built out of the shear strains on the di"erentslip systems:

!pl !X

i

!#i$M#i$, M#i$ ! 1

2bb#i$ & n#i$ " n#i$ & b#i$h i

: #2$

Here the index i distinguishes the di"erent slip systems, !(i) are the respective scalarshear strains, and b is the modulus of the Burgers vector (for simplicity assumedthe same for all slip systems). The projection tensors M#i$ are symmetrized tensorproducts of unit vectors in the respective slip plane normal and slip directions.

The driving force for slip on a given slip system is the respective resolvedshear stress "(i), which is the inner product of the stress tensor D and the projectiontensor M#i$:

"#i$ ! M#i$ ' D: #3$

188 M. Zaiser

Downloaded By: [Karlsruher Inst fur Technologie Kit] At: 14:00 9 December 2010

To specify the elastic–plastic material behaviour, one has to provide constitutiverelations which relate the stress to the plastic strain and possibly to the strain rateand other variables. In crystal plasticity, these are relations between scalar variables(shear strains, resolved shear stresses). To avoid cumbersome notation, in thefollowing we adopt a strictly scalar formulation by focusing on shear deformationon a single slip system. Accordingly, we drop the superscript #i$.

Constitutive relations The simplest elastic–plastic models continue the elastic stress–strain relation into a relationship between the stress and the strain in the plasticregime. The basic type of such rate-independent constitutive models is commonlycalled ideal plasticity (figure 1, left). In this case, the plastic strain in a material elementremains zero unless the stress reaches a critical value "y (yield stress) and then increasesindefinitely. This corresponds to the assumption of a material that cannot support anyshear stresses above the yield stress: at yield the solid e"ectively turns into an idealfluid; upon unloading it immediately re-assumes the properties of a linear elastic solid,while the permanent shear deformation remains (dashed line in figure 1, left).

A generalization of this type of constitutive behaviour is to assume that, in theplastic regime, the stress required to deform a material is an increasing function ofstrain (strain hardening). In the stress–strain graph the onset of plasticity in this casecorresponds to a change in slope (figure 1, right). The slope of the stress–strain graph"#!$ in the plastic regime is called the strain hardening coe"cient # or, in continuummechanics language, the tangent modulus. Again, it is important to keep in mindthat the elastic and plastic regimes not only di"er in the slope of the stress–straingraph, but that the physical processes are fundamentally di"erent (reversible vs.irreversible deformation), as becomes again evident upon unloading (dashed linein figure 1, right).

A di"erent class of models considers plasticity as a time-dependent flow process.Linear viscoplasticity assumes that the shear strain rate _! is zero up to a critical stress(again the yield stress) and then increases linearly with stress (figure 2):

_! ! 1

$

#j"j% "y$ sign#"$, j"j > "y,

0 else:

!#4$

!

!y

""pl

!

!y

"pl "

#

Figure 1. Di"erent types of rate-independent plasticity; left: ‘ideally plastic’ behaviour;right: plasticity with strain hardening.

Scale invariance in plastic flow of crystalline solids 189

Downloaded By: [Karlsruher Inst fur Technologie Kit] At: 14:00 9 December 2010

In this equation, the sign function indicates that the direction of shearing is dictatedby the sign of the driving stress, whereas the velocity depends on the excess of thedriving over the yield stress. $ is a viscoplastic rate coe!cient. A viscoelastic solidbehaves like a solid for stresses below and like a Newtonian liquid for stresses abovethe yield stress (‘yield-stress liquid’).

In a viscoplastic solid, the stress required for deformation is a function of thedeformation rate (‘flow stress’). In particular, if we impose a constant deformationrate _!0, from equation (4) the stress for steady-state deformation becomes

"f# _!$ ! "y " $ _!0, #5$

i.e. the flow stress increases with increasing deformation rate. Rate-independentplasticity is recovered in the limit of small $ ( "y= _!0.

Linear viscoplasticity can be generalized to account for strain hardening, byassuming that the critical stress at which flow initiates is an increasing function ofthe plastic strain, "y ! "y#!$ in equation (4). Other generalizations may includenonlinear relationships between stress and strain rate, and the inclusion of additionalvariables such as temperature, or of internal variables describing the materialmicrostructure.

Plastic instabilities and stable plastic flow Under ‘normal’ deformation conditions,a strain hardening viscoplastic material responds to a homogeneous driving stressin a spatially homogeneous manner. Under certain conditions, however, smallperturbations of a homogeneous flow mode may become undamped, and one isdealing with a plastic instability. We consider linear viscoplastic flow with a genericstrain dependence of the yield stress. In the plastic regime we have from equation (4)

_! !" % "y#!$

$, #6$

where " is now understood as an externally applied shear stress which we takewithout loss of generality to have positive sign. One may now consider the evolutionof small local perturbations %! of some homogeneous deformation mode !0(t) – forinstance, !0#t$ ! _!0t for a constant imposed strain rate _!0, or the response !0(t) to

"2

"1

" –> 0

"

!y ! "

!

!y

Figure 2. Linear viscoplasticity; left: strain rate vs. stress; right: stress–strain curves fordriving at di"erent rates _!1 > _!2.

190 M. Zaiser

Downloaded By: [Karlsruher Inst fur Technologie Kit] At: 14:00 9 December 2010

a stress " ! _"t ramped up at a constant rate. The evolution of perturbations is ineither case given by

% _! ! % ##!0$$

%!, # !@"y@!

, #7$

provided that the external stress is unchanged by the perturbation. Perturbationsbecome undamped if either the tangent modulus # or the viscoplastic coe!cient $turn negative. The first case is referred to as strain softening, the second as strain ratesoftening instability. This terminology can be rationalized from equation (5) for theflow stress: In case of strain softening the partial derivative @"f=@!j _! and in case ofstrain rate softening the partial derivative @"f=@ _!j! become negative.

Plastic instabilities give rise to various kinds of interesting phenomena like non-linear oscillations, travelling waves, deformation localization, patterning and chaos.An overview of these phenomena can be found elsewhere [2, 3]. Generally speaking,instability of the homogeneous deformation mode reveals the presence of internallength and time scales (for the role of internal length scales in plastic instabilities andthe related problems for constitutive modelling, see, e.g. Aifantis [11, 12]; for theproblem of internal time scales and the relationship between strain rate softeningand Hopf bifurcations, see Hahner and Zaiser [13]).

In the context of the present paper, however, we are interested in collectivephenomena during ‘stable’ plastic deformation. In this context it is useful to comeback to the simplest plasticity model: that of a rate-independent ideally plasticmaterial. From the point of view of plastic stability/instability, deformation ofsuch a material is marginally stable both in the strain and strain rate softeningsense, since both the hardening and viscoplastic coe!cients are by definitionequal to zero. Hence, fluctuations may become relevant on all scales, and it is notastonishing that di"erent kinds of critical phenomena may be observed as soon asone approaches the yield stress. Of course, rate-independent ideal plasticity doesnot exist in real materials – but it is not a completely o"-the-mark approximationeither: If we measure stresses in units of the shear modulus G, then the characteristichardening rates of most crystalline materials are small (typically 10%4 <#=G < 10%2). The same is true for the rate-dependent contribution to the flow stress,which is small at least in fcc and hcp metals and for deformation rates accessible instandard deformation testing. In consequence, deforming crystals can often be envi-saged as slowly driven non-equilibrium systems whose internal dynamics are char-acterized by intermittent jumps between metastable near-equilibrium configurationsof the defect microstructure: Most of the time, almost nothing is happening in mostof the crystal volume, while plastic flow occurs through intermittent bursts of activitywhich are associated with collective rearrangements in the microstructural patternand lead to sudden increments in strain [4, 14]. To better understand the nature ofthese rearrangements, it is necessary to envisage plasticity on the level of crystaldislocations.

1.2. Crystal plasticity on the dislocation level: yield stressand depinning transition

Dislocations and plasticity The physicist’s approach towards plasticity has alwaysfocused on the elementary mechanisms of plastic flow in a material with a given

Scale invariance in plastic flow of crystalline solids 191

Downloaded By: [Karlsruher Inst fur Technologie Kit] At: 14:00 9 December 2010

atomic structure, rather than on constitutive equations for the flow of a continuousmedium. The elementary mechanism of crystallographic slip is not the rigid sliding oflattice planes above each other, but the expansion of a slipped area. The boundary ofa slipped area is a one-dimensional lattice defect: a dislocation. A dislocation line ischaracterized globally by the slip plane and by the Burgers vector of the correspond-ing slip system, and locally by a unit tangent vector t characterizing the linedirection. Depending on the angle between t and b, it is conventional to distinguishedge (t ? b), screw (t k b) and mixed segments. A shear stress " acting in the disloca-tion slip system creates a force per unit length on the dislocation (Peach–Koehlerforce, [15]). The component of this force in the dislocation glide plane (with normalvector n) is given by

FPK ! "b)t* n+: #8$

This force perpendicular to the dislocation line acts as the driving force fordislocation glide: it moves the dislocation such as to shear the material in thedirection imposed by the slip geometry and the sign of the stress ".

The lattice around a dislocation is distorted: dislocations possess long-rangestress fields. The stress field of a straight dislocation is given by

"D#r$ !Gb!##$

r, #9$

where # is the angle in the plane perpendicular to the dislocation, r is the verticaldistance from the dislocation, and the function ! has zero average. The stress field ofa curved dislocation can, at least outwith the immediate vicinity of the dislocationline, be considered as a superposition of stress fields of short straight segments,

"S#r$ !Gb"##,&$ds

jrj2, #10$

where r is now the vector connecting the segment to the point under consideration,ds is the length of the segment and " is another angle-dependent function whoseaverage over the unit sphere vanishes (for explicit expressions, see [16]). The long-range stresses associated with dislocations or dislocation segments lead in the case ofcurved dislocations to self-interactions (which tend to keep the dislocation straight),and in general to interactions between di"erent dislocation lines. Plasticity on thedislocation level corresponds to the collective dynamics of a system of interactingelastic lines under the action of external driving forces.

Leaving for the moment the question of dislocation creation aside (mostcrystalline solids contain appreciable densities of dislocations resulting from crystalgrowth and preparation history), a crystal will yield plastically if the applied stress issu!cient for the sustained motion of a generic lattice dislocation. In general, thismotion will in turn increase the dislocation density, as the expansion of dislocationloops increases the dislocation length contained in the crystal. (The generation ofdislocations ex nihil requires stresses which are orders of magnitude above thoserequired to move existing dislocations; this is a process which is hardly relevantfor plasticity except in extreme cases such as the deformation of dislocation-freewhiskers.)

192 M. Zaiser

Downloaded By: [Karlsruher Inst fur Technologie Kit] At: 14:00 9 December 2010

Hence, from the dislocation point of view yielding is the onset of sustainedmotion of a generic dislocation: Yielding is dislocation depinning. We will firstconsider the depinning of a single dislocation (or a hypothetical population ofnon-interacting dislocations), which reduces to the well-investigated problem ofa single one-dimensional elastic manifold moving through a two-dimensionaldisordered medium. Even though this picture is not fully realistic (real dislocationsdo interact over long distances), it will be useful for introducing relevant conceptsand notations of the literature on depinning transitions.

Depinning transition of a single dislocation We envisage a dislocation gliding in thez! 0 plane. The dislocation is assumed to be on average straight and to run alongthe x direction. The Burgers vector is b ! bey (edge dislocation). A shear stress " isapplied to the considered volume element from outside and creates an externaldriving force acting on the dislocation. If the dislocation line is not compeletelystraight, elastic interactions between di"erent segments will create a stress thattends to straighten the dislocation; for small perturbations y(x) of a straight linethis stress can be written as

"self#x$ !"y#x$ % y#x0$# $

#D#x% x0$dx0, #11$

where the stress kernel #D decreases in space like 1=jx% x0j3 (for explicit expressions,see [17]). In the theory of depinning, it is usual to classify elastic kernels in termsof their long-wavelength behaviour in Fourier space. A 1/r3 kernel acting on aone-dimensional manifold scales like jkj2 with logarithmic corrections, which putsthe problem into the realm of local elasticity: This is why the self-interaction ofa dislocation can be represented to a good approximation by a local line tension.

In addition to its self-interaction, the dislocation interacts with other defects(atomic defects or other dislocations) which create an e"ective pinning force.We assume a random defect arrangement which gives rise to a spatially fluctuatinginternal stress field %"#r$ with zero average and short-range correlations:

h%"#r$i ! 0, %"#r$%"#r" r0$% &

! %"2% &

'jj%#x0$ f"# y0$, #12$

where f" is a short-ranged correlation function of characteristic range '?, and 'k and'? are correlation lengths of the fluctuating stress field in the directions parallel andperpendicular to the dislocation, respectively. The pinning defects are assumed to beimmobile (quenched disorder).

Moving dislocations experience a friction force due to scattering of phonons andelectrons. Since the e"ective mass of dislocations is generally small, their motion isunder most circumstances overdamped, i.e. the velocity is proportional to the actingforce. For a straight dislocation with small perturbations, the equation of motion ofthe dislocation line becomes

1

$Db@ty#x$ ! " "

"y#x$ % y#x0$# $

#D#x% x0$dx0 " %"#x, y$, #13$

where $D is the dislocation drag coe!cient. Equation (13) is a variant of thequenched Edwards–Wilkinson equation describing the motion of an elastic interface(elasticity mediated through the kernel #D) through a disordered medium

Scale invariance in plastic flow of crystalline solids 193

Downloaded By: [Karlsruher Inst fur Technologie Kit] At: 14:00 9 December 2010

(characterized by the quenched random field %"#x, y$) under the action of an externaldriving force. Since this problem has received extensive attention in the literature(see the reviews by Leschhorn et al. and by Fisher [18, 19], or the more recent worksof Le Doussal and co-workers [20, 21]), we here only summarize the main results indislocation language:

. Below a critical driving stress "c, the dislocation gets asymptotically pinned(v ! h@tyi ! 0 for t ! 1 and " < "c). The magnitude of the critical stressdepends on the statistical properties of the pinning field %", and on the relativemagnitude of the pinning and self-interactions. Practically all the metallurgicalliterature on the problem is devoted to evaluating this critical stress for thevarious types of pinning fields that may be encountered in di"erent metals andalloys. Some classical estimates can be found in the works of Labusch, Larkinand Friedel [15, 22–24]. While the pinning strength of a given disorderedmicrostructure is of paramount importance for applied metallurgy (dislocationpinning may determine the strength of the turbine blades in your aircraft), wewill adopt a statistical physicist’s stance and focus on the universal dynamicalproperties at the depinning transition, for which the yield stress (being anon-universal quantity anyway) is of little relevance.

. At the depinning stress "c, a dynamic phase transition occurs from a pinned toa moving phase. This transition is second-order-like, with the mean velocity ofthe dislocation – which plays the role of an order parameter – increasing like

v / #" % "c$( #14$

where ( is called the velocity exponent. Well above the critical stress(for " , h%"2i1=2), the disorder becomes irrelevant and the dislocation velocityincreases linearly with stress. This situation is schematically depicted in figure 3.

. Near the critical stress the dislocation assumes a self-a!ne lineshape.A self-a!ne curve y(x) is statistically invariant under the transformationx ! )x, y ! )*y, where * is the roughness exponent. Scale invariance isdelimited by an upper correlation length ' which diverges as one approachesthe critical stress,

' / j" % "cj%+, #15$

with the correlation length exponent +. As a consequence of the self-a!nebehaviour, the mean height di"erence between two points along the line scaleslike

jy#x$ % y#x" l $j% &

/ l*fy#l='$, #16$

where the scaling function fy has the asymptotic properties fy#u$ ! 1, u ( 1and fy#u$ ! u%*, u , 1. Roughening of an initially straight dislocation startson small scales, over domains of size l / t1=z where z is called the dynamicexponent. Near the critical stress, the transient dynamics is described by theFamily–Vicsek scaling form [25]

y#x$ % y#x" l $'' ''% &

! l*fyl

t#1=z$

( ), #17$

194 M. Zaiser

Downloaded By: [Karlsruher Inst fur Technologie Kit] At: 14:00 9 December 2010

which is also observed in a wide class of other problems including the thermalroughening of elastic manifolds and diverse models of surface growth.

. Near the critical stress, the motion of the dislocation proceeds throughintermittent avalanches during which segments rapidly sweep forward beforethey get trapped again. In the pinned phase, release of an avalanche from atrapped configuration is contingent upon a small increase in the external stress.In the moving phase, on the other hand, the system never gets completelytrapped and the definition of an ‘avalanche’ therefore requires the introductionof a velocity threshold. In either case, the avalanches exhibit a power-law sizedistribution,

p#s$ ! s%,s fs#s=s0$, #18$

where the avalanche size s corresponds to the swept area, ,s is the avalancheexponent, and the scaling function fs (fs#u$ ! 1 for u ! 0, fs#u$ ! 0 foru ! 1) decays for large u faster than algebraically. The cut-o" of thepower-law distribution corresponds to an avalanche of characteristic extension' in the x direction, hence s0 - '1"* / j" % "cj%+#1"*$. The duration of anavalanche is related to its extension in the x direction through the dynamicexponent, t / xz, and to its size by t / sz=#1"*$.

This type of behaviour is found in many physical situations where elasticmanifolds move through some kind of pinning field. Examples include dislocations[17], vortex lines in superconductors, cracks [19], domain walls in ferromagnets [26],grain boundaries [27], contact lines in wetting, and sliding interfaces in friction [28].In the following paragraph, we give scaling relations as well as a ‘catalogue’ ofcritical exponents for di"erent dimensionality of the interface and range of its elasticself-interaction.

Critical exponents and scaling relations for depinning transitions We consider ad-dimensional interface moving in d" 1 dimensions (for a dislocation moving on

<v>

(!$!c)%

!c !

Figure 3. Stress–velocity relation for a depinning dislocation.

Scale invariance in plastic flow of crystalline solids 195

Downloaded By: [Karlsruher Inst fur Technologie Kit] At: 14:00 9 December 2010

its glide plane, d! 1). We exclude overhangs, so the interface can be characterized bya single-valued function. The elastic self-interaction of the interface is characterizedby an elastic kernel ##r$ (R 2 d$ whose Fourier transform scales like jkja for jkj ! 0,i.e. in real space it decays like jrj%d%a, or possibly faster for a! 2. The interfacemoves under the action of a generalized force (or stress) " across a time-independentrandom force field of zero average and with short-range spatial correlations.

The main characteristics of the dynamics have been discussed in the previoussection for the special case of an isolated dislocation. Numerical values for thevelocity, correlation length and roughness exponents are compiled in table 1,including results from functional renormalization (Le Doussal et al. [21]) and fromsimulations (references cited). We also include values for the mean-field case whichbecome valid above the critical dimension dc ! 2a [19, 26].

In the following we compile some scaling relations that may be useful for thelater discussion. All relations will be motivated by intuitive scaling arguments; fora rigorous derivation the reader is referred to the literature.

. A relation between the dynamic and velocity exponents is found by noting thatthe mean velocity of the interface is governed by the largest jumps, duringwhich segments of linear extension ' move over distances '*. The time it takesthe interface to reach an (almost) pinned configuration is t / 'z, and' / #" % "c$%+ in the moving phase. Hence the velocity exponent obeys thescaling relation

( ! +#z% *$: #19$

Table 1. Critical exponents for interface depinning as a function of the parameters d and a;functional renormalization results (FRG, expansion in " ! dc % d $ after Le Doussal et al. [21];

mean-field results after [26].

d a FRGO#"$ FRG O#"2$ Simulation

Roughness 1 2 1.00 1.43 1.25. 0.05 [18]* 2 2 0.66 0.86 0.75. 0.02 [18]

3 2 0.33 0.38 0.34. 0.01 [18]1 1 0.33 0.47 0.34. 0.02 [29]

MF 0

Correlation length 1 2 0.75 0.98 1.00. 0.05 [30]+ 2 2 0.67 0.77 0.77. 0.04 [31]

3 2 0.58 0.611 1 1.33 1.58 1.52. 0.02 [29]

MF 2/d

Velocity 1 2 0.67 0.31 0.25. 0.03 [18]( 2 2 0.78 0.62 0.64. 0.02 [18]

3 2 0.89 0.85 0.84. 0.01 [18]1 1 0.78 0.59 0.68. 0.06 [29]

MF 1

196 M. Zaiser

Downloaded By: [Karlsruher Inst fur Technologie Kit] At: 14:00 9 December 2010

. The avalanche exponent can be related to other exponents by considering theaverage susceptibility which is proportional to the mean avalanche size,- ! @hyi=@" / hsi. On the one hand, - / '*='1=+, hence

- / #"c % "$%#1"+*$: #20$

On the other hand, the mean avalanche size is

hsi / s2%,0 , s0 / #"c % "$%+#d"*$: #21$

Combining these relations, we find the exponent relation [26, 32]

, ! 2% 1" *+

+#d" *$: #22$

. Additional relations can be found for the relation between size and duration ofan avalanche, and for the relaxation of the mean velocity near the criticalstress. The size of an avalanche of linear dimension x is s ! xd"*, and thecorresponding time scale is t ! xz, hence

t / sz=#d"*$: #23$

For the velocity relaxation near the critical point we find the scaling v / x*%z

and with t / xz we get

v / t2=z%1 ! t(=#+z$: #24$

In the following these exponents and scaling relations will appear in di"erentcontexts. In all of these the mean position of the ‘interface’ corresponds to a strain-like variable (for instance, the mean distance hyi travelled by a dislocation corre-sponds, for a hypothetical ensemble of non-interacting dislocations of density ., tothe macroscopic strain ! ! .bhyi). The word ‘interface’ should be taken with a grainof salt: whereas a single dislocation clearly is an interface between a slipped anda non-slipped region, and a dislocation wall is an interface between two regions ofdi"erent lattice orientation, the intuitive notion of an interface becomes much morespurious if one is dealing with a dislocation procession or pile-up. In section 3 wewill even encounter a model where the ‘interface’ coordinates are the Cartesiancoordinates of a volume element in the deforming crystal, and the direction intowhich this interface is ‘moving’ corresponds to the local shear strain. The scalingrelations and exponents characterizing the dynamics are una"ected by such semanticsubtleties.

2. Experimental investigation of fluctuation phenomena in plastic flow

2.1. Acoustic emission measurements

2.1.1. Experimental methodology. As dislocations move during plastic deforma-tion, they lose energy to the phonon and electron systems in the crystal. In manysituations, the resulting drag force is so large that dislocation motion e"ectivelyproceeds in an over-damped manner. If dislocation motions are su!ciently rapid,the energy loss cannot be exclusively envisaged in terms of dissipation and heat

Scale invariance in plastic flow of crystalline solids 197

Downloaded By: [Karlsruher Inst fur Technologie Kit] At: 14:00 9 December 2010

generation, but part of the energy is emitted in the form of travelling acoustic waveswhich can be detected as an acoustic emission signal. Therefore, acoustic emissionrecordings may be used as a tool for monitoring dislocation activity during plasticdeformation.

A major problem in the interpretation of acoustic emission signals is, however,to establish the relation between the observed voltage record and the underlyingdislocation processes. The transmission function between the acoustic source andthe recorded signal is in general very complicated and, more importantly, the sourcecharacteristics themselves have to be understood and related to the amplitude of theemitted acoustic wave. Most investigations of source characteristics envisage theexpansion of a compact dislocation loop [33, 34], or a procession of loops emittedfrom a common source [35]. Generally it is found that the amplitude of the emittedacoustic wave is proportional to the velocity v of the expanding loop: hence theacoustic power, which is the square of the amplitude, is proportional to v2.In general, however, acoustic emission may be due to the simultaneous motion ofmany dislocations or dislocation segments, rather than the expansion of a singleloop. Rouby and co-workers [33, 34] analyse the uncorrelated superposition ofevents coming from di"erent sources as a paradigm for a ‘continuous’ AE signal,as well as a sequence of closely correlated events from one source which they use as aparadigm for a ‘discrete’ AE burst. In reality, the situation may be more complicatedsince the AE signal during a deformation avalanche may be produced by temporallycorrelated dislocation motions at di"erent locations which, owing to the long-rangeinteractions characteristic of dislocation systems, may be distributed according tocomplicated spatial patterns with long-range correlations (see section 3.2). For aburst during which N dislocation segments of characteristic length lmove collectivelyat locations close to each other and with a constant velocity v, the peak acousticemission amplitude is [36]

A ! KNlhvir

/ Kl

r_!: #25$

In this equation, r is understood as the distance from the source to the acoustictransducer and K is a constant containing material properties (sound velocities) aswell as transducer properties. It is seen from equation (25) that for burstlike emissionthe acoustic emission amplitude is essentially proportional to the instantaneousstrain rate.

2.1.2. Acoustic emission in single- and polycrystals of ice. Very systematic and com-prehensive investigations of the statistics of acoustic emission bursts have beenperformed by Weiss and co-workers on ice single- and polycrystals [6, 7, 36–41].Ice may be considered an ideal ‘model material’ for AE studies of crystal plasticityfor several reasons [38]: (i) Even at comparatively low stresses and temperatures closeto the melting point, plastic flow of ice proceeds by glide of dislocations (in mostother materials, at high temperatures and low stresses di"usional deformationmechanisms become predominant). (ii) Single crystals of hexagonal ice Ih exhibitvery pronounced plastic anisotropy, as deformation occurs essentially by glide onbasal planes. As a consequence, deformation by dislocation glide on a single slipsystem is robust in comparison with metals, where single slip is confined to very

198 M. Zaiser

Downloaded By: [Karlsruher Inst fur Technologie Kit] At: 14:00 9 December 2010

small strains. (iii) Transparency of the samples allows us to verify that AE activityis not due to microcracking. (iv) Excellent acoustic coupling can be achieved byfreezing the transducers onto the sample surface.

In their studies, Weiss and co-workers focus on creep at elevated temperatures(/%10'C) and low stresses (/1MPa). They observe an intermittent acousticemission signal composed of discrete AE bursts and systematically investigate thestatistics of the bursts and their temporal and spatial correlations.

Avalanche statistics In their investigations, Weiss et al. characterize the burstlikeAE signal from ice single- and polycrystals both in terms of the peak amplitudesA ! max)A#t$+ and in terms of the acoustic energy E !

*BA

2#t$dt where B denotes acompact interval over which the AE intensity exceeds a given threshold (of course,one has to check whether the statistics is robust against changes of the thresholdvalue). For single crystals, the observations indicate scale-free distributions of burstamplitudes and energies (see figure 4),

p#E $ / E%,E , p#A$ / A%,A , #26$

with exponents ,E - 1:6 and ,A - 2:0 that are approximately independent on stress,strain, and temperature [40]. The distribution of time intervals $t between AE eventswas also investigated. A cumulative distribution P#$t$ / $t%1 (i.e. p#$t$ / $t%2

for the non-cumulative distribution) was reported by Weiss and co-workers in [37](insert in figure 4).

0 2 4 6 8 10$10

$5

0

5

1 10 1001

10

100

&E = $1.6

! = 0.086 MPa! = 0.067 MPa! = 0.037 MPa! = 0.030 MPa

Log 1

0P(E

)

Log10(E)P

('t

)

't [s]

Figure 4. Energy distribution of AE events recorded during creep deformation of ice singlecrystals; temperature T ! 263K, resolved shear stresses on the basal plane as indicated in theinset, after Miguel et al. [6]; insert: cumulative distribution of time intervals between AE eventsrecorded during creep of an ice single crystal at a resolved shear stress of 0.58MPa, after Weisset al. [37].

Scale invariance in plastic flow of crystalline solids 199

Downloaded By: [Karlsruher Inst fur Technologie Kit] At: 14:00 9 December 2010

Investigations on polycrystals show an altogether more complex picture [40, 41].Unlike single crystals where the amplitude and energy distributions of AE bursts arescale-free over the entire accessible amplitude/energy range, the burst amplitudes andenergies in AE signals of polycrystals have upper limits which increase with increa-sing grain size. Furthermore, the avalanche exponents are reduced in comparisonwith single crystals (,A - 1:35 in polycrystals). It has been inferred from theseobservations that grain boundaries may act as e!cient barriers to the propagationof slip avalanches. The existence of such barriers may lead to substantial stressconcentrations (intergranular stresses), and it has been suggested that such overs-tresses may explain the observed decrease in the avalanche exponent, as they mayhelp small avalanches to coalesce into larger ones, up to a scale governed by thegrain size [40, 41]. Even more complicated behaviour has been observed in poly-crystals with a bimodal grain size distribution containing a few very large grains: Inthese polycrystals, a single-crystal exponent ,A - 2 at small avalanche sizes and apolycrystal exponent ,A - 1:35 at larger sizes have been observed simultaneously.

Spatial patterns and space–time correlation of deformation avalanches By usingmultiple acoustic transducers, Weiss and Marsan [7] investigated the spatial locationof acoustic emission ‘events’ in ice single crystals. By recording the arrival times ofthe acoustic signal at di"erent locations and using spatial triangulation, they wereable to locate the points of origin of the AE signals emanating from large deforma-tion events with an accuracy of about 400 mm, limited by the time resolution of therecording device. They used the correlation integral method to analyse the spatialpattern of the points of origin of the AE signals (i.e. the points where deformationavalanches have initiated). Their results indicate a self-similar pattern with a correla-tion dimension of DF - 2:5. The observed scaling regime extends over about 1.5orders of magnitude; it is limited from above by the specimen size and from belowby the spatial resolution of the recording technique.

10$3 s

Figure 5. Acoustic emission signal (amplitude vs. time) recorded during compression testingof an Al polycrystal; after Imanaka et al. [42].

200 M. Zaiser

Downloaded By: [Karlsruher Inst fur Technologie Kit] At: 14:00 9 December 2010

The same investigation also revealed a space–time coupling in the avalanchedynamics: Avalanches that are close in the sequence of events tend also to be closerthan average in space. This observation complements studies of the temporalcorrelation of deformation events: An analysis of the temporal correlation functionrevealed temporal clustering of deformation events [38] and a more detailedinvestigation showed an enhanced ‘aftershock activity’ after big deformationavalanches, with an average number NA of aftershocks that was found to beproportional to a power of the avalanche amplitude, NA / A0:6 [39]. These findingsprovide evidence for the existence of a coupling between di"erent deformation eventsthat leads to their clustering both in space and in time.

2.1.3. Acoustic emission in metals and alloys. Acoustic emission studies have beenreported on various pure metals and alloys [33, 34, 42–44]. The observed AE signalsinclude both discrete bursts and continuous noise, sometimes occurring simulta-neously in the form of discrete spikes with a continuous background [43].Unfortunately, in the older literature there exist few statistical investigations ofburst characteristics, e.g. in terms of amplitude or energy distributions. Instead,the traditional paradigm of plastic flow as a more or less continuous process ledmany researchers to focus on the continuous background from which the discontin-uous bursts were seen as a kind of pathological exception. For instance, Kiesewetterand Schiller [43] report discrete dislocation bursts superimposed on a continuousbackground signal but attribute only the continuous background to dislocationmotion. In line with this practice, most AE studies attempt to establish relationsbetween plastic flow characteristics and parameters of the AE signal that areaveraged over the fluctuations of the dynamics, such as the mean intensity or, incase of burst-like signals, the mean burst rate.

Very recently, Richeton et al. have provided a statistical investigation of theacoustic emission bursts that are generically observed in deformation of hexagonallyclose-packed (hcp) metals and alloys [45]. This investigation demonstrates that AEbursts in single crystals of Cd and ZnAl exhibit scale-free energy distributions withexponents ,E - 1:5 that are very similar to those observed in ice single crystals. Alsoother findings, such as the observation of temporal correlations between AE bursts,were analogous. This result is remarkable in several respects: (i) The experiments onhcp single crystals were conducted in tension at constant crosshead velocity, which isa quite di"erent loading mode from the constant-stress creep conditions under whichthe ice results were obtained. (ii) The same scale-free distribution of burst energieswas found in hardening stage I (deformation by dislocation glide on a single slipsystem), in hardening stage II (preferential deformation on a single slip system, butstrong forest hardening because of additional dislocation activity on secondary slipsystems), and for crystal orientations where deformation proceeds mainly bytwinning. These findings demonstrate a remarkable robustness of the scale-freebehaviour of AE signals in plastically deforming crystals and indicate thatintermittent ‘crackling’ noise [46] may be a universal signature of deformation bycrystallographic shear (slip or twinning).

Scale invariance in plastic flow of crystalline solids 201

Downloaded By: [Karlsruher Inst fur Technologie Kit] At: 14:00 9 December 2010

2.2. Deformation-induced surface patterns

Plastic deformation leads to characteristic surface phenomena which can be used tomonitor the flow process and gain information on plastic flow patterns. Along thelines of intersection between the active slip planes and the surface, movingdislocations leave behind them atomic-scale surface steps (‘slip lines’) which canbe considered as records of the dislocation movements which have producedthem. Characterization of plastic deformation using surface micrographs is an‘old’ experimental technique which dates back to the 1950s. With the advent oftransmission electron microscopy, surface-based techniques fell somewhat out offavour, since dislocation motion near free surfaces is inevitably a"ected by surfacee"ects – for instance, the presence of a free surface modifies the stress field such thatdislocations near surfaces experience image forces and may annihilate at the surface,leading to the formation of a soft dislocation-depleted surface layer with a width ofa few (bulk) dislocation spacings. The problem of surface-induced artefacts is mostsignificant if one wants to study small-scale features (arrangement and motionsof individual dislocations or dislocation groups) but may be less critical if one islooking for scale-free features.

As far as scale-free patterns in plastic flow of solids are concerned, surface-basedtechniques have one distinct advantage: Surface investigations give the possibilityto characterize deformation-induced surface patterns from the atomic up to themacroscopic scale in terms of a single type of experimental information (surfaceheight, positions of surface steps). Bulk techniques operating on di"erent scales,on the other hand, have to cope with the di!culty that the di"erent techniques(e.g. transmission electron microscopy and X-ray topography) yield qualitativelydi"erent types of information. Data obtained by di"erent techniques can thereforenot be simply stitched together to yield a comprehensive multiscale characterization.

In view of the availability of experimental techniques covering features from theatomic to the macroscale, and the simplicity of compiling information from di"erentscale regimes into a comprehensive picture, surface techniques seem particularlysuited to monitor the multiscale organization of plastic deformation throughdi"erent stages of the deformation process and to detect scaling laws and scale-free features. This may be done by looking at the distribution of slip lines on thesurface, which give local information on the deformation process in terms of thepositions where individual dislocations have left the surface producing units of slip,or by looking at surface profiles which yield the corresponding integral informationabout the global slip pattern.

2.2.1. Slip-line patterns. Slip lines emerging under single-slip conditions formstriated patterns of parallel lines (figure 6), and it was suggested already in the1980s that the points of intersection of the slip lines with a line drawn normal tothem might form some kind of randomized Cantor set. This proposition wasfollowed up by Sprusil and Hnilica [47] and Kleiser and Bocek [48]. Sprusil andHnilica [47] tried to deduce a fractal dimension by determining the mean slip linespacing from micrographs of di"erent magnification. This is methodologicallyspurious, as discussed in [10] in relation with the fractal analysis of dislocationcell patterns. Kleiser and Bocek [48], on the other hand, provided a systematic

202 M. Zaiser

Downloaded By: [Karlsruher Inst fur Technologie Kit] At: 14:00 9 December 2010

investigation using various techniques (gap width distribution, box counting, andcorrelation integral) to determine the fractal dimension of slip line patterns.Their findings may be summarized as follows:

. Slip lines on the surface of a Cu single crystal that were generated withina narrow strain interval (0:59 < ! < 0:69) exhibit a statistically self-similarpattern over a range of scales between typically 0.06 and 2 mm. Theset of intersection points with a normal line has a fractal dimension ofD - 0:4%0:7, depending on the method used.

. Slip lines accumulating over a larger strain interval from the beginning ofdeformation form a more or less homogeneous pattern without clear evidenceof self-similar behaviour.

These findings indicate long-range correlated fluctuations in the flow processwhich, however, persist only over limited intervals of time (or strain). The investiga-tions of Kleiser and Bocek, and Sprusil and Hnilica, were based upon the analysis ofoptical surface micrographs dating from the 1950s and 1960s. A problem with thesemicrographs is that they do not allow us to quantitatively resolve the height of theslip steps, i.e. the number of dislocations that have exited the crystal along a givenslip line or, equivalently, the local strain concentration. The observed long-rangecorrelations in the slip-line pattern can therefore not be directly translated intocorrelations in the strain pattern. A semi-quantitative analysis was provided byKleiser and Bocek who estimated the slip step height from the width of slip linesvisible on surface micrographs and used this to ‘weight’ the lines. Fractal dimensionsof the resulting weighted patterns were somewhat higher than those of slip-linepatterns with all visible lines given equal weight. A more quantitative analysiscould nowadays be provided by using atomic-resolution AFM to determine theheight and spacing of surface steps, but this remains still to be done.

2.2.2. Slip-line kinematography. By in situ optical observation of the surface ofa plastically deforming crystal (so-called slip-line kinematography), it is possible togain information about the dynamics of plastic flow. An overview of experimental

Figure 6. Slip lines on the surface of a Cu-30 at% Zn single crystal deformed in tensionat 77 K to a strain of 19.4%. Courtesy of H. Neuhauser.

Scale invariance in plastic flow of crystalline solids 203

Downloaded By: [Karlsruher Inst fur Technologie Kit] At: 14:00 9 December 2010

methods can be found in the review by Neuhauser [49]. Because of the necessity ofkeeping in focus a small surface window which is imaged with high magnification,the technique is not suited for studying the evolution of large-scale deformationpatterns, but it can give useful information about the temporal evolution of sliplines or slip-line clusters (slip bands).

Clustering of slip is pronounced in alloys exhibiting so-called planar slip wheredislocations tend to move in large processions (pile-ups). In this case, one is dealingwith the dynamics of linear or almost linear dislocation arrays, rather than indivi-dual dislocations. Scale-free behaviour has been observed in the growth kinetics ofsurface steps, where the growth rate has been found to decay in inverse proportionwith the time elapsed from the onset of step growth (figure 7, [50]).

For a moving pile-up consisting of roughly equally spaced dislocations, the slipstep growth rate is proportional to the pile-up velocity. Since often only a smallnumber of slip steps are growing at a time [49], one may therefore attempt to relatethe observed time dependence of slip step growth to the velocity relaxation of a singlepile-up. The double-logarithmic plot in figure 7 indicates relaxation of the growthrate (the pile-up velocity) according to v / t%1.0:1 over six decades.

According to the relations given in the introduction, a planar dislocation arrayin a three-dimensional crystal falls into the class d ! 2, a ! 1, i.e. the depinningtransition of such arrays exhibits mean-field behaviour. For the velocity relaxationnear the critical point one then expects according to equation (24) and table 1 anexponent (=#+z$ ! 1, which is in line with the experimental data. The length of thescaling regime may be taken as an indication that driving of the dislocation arraysoccurs at stresses very close to the critical one.

10$6 10$5 10$4 10$3 10$2 10$1 100 101 102

time [s]

10$6

10$5

10$4

10$3

10$2

10$1

100

101

102

slip

line

gro

wth

rat

e [m

m/s

]

Figure 7. Growth rate of slip steps on the surface of Cu-30 at% Zn deformed at roomtemperature as a function of the time passed after growth has started; after [50]. The lineis a power law with exponent %1.

204 M. Zaiser

Downloaded By: [Karlsruher Inst fur Technologie Kit] At: 14:00 9 December 2010

2.2.3. Surface roughening in single- and polycrystals. Long-range correlations inthe pattern of surface steps can be detected indirectly through analysis of surfaceprofiles, even if the experimental resolution is not su!cient to resolve individualsurface steps. The relation between one-dimensional surface profiles evolving froman initially smooth surface, and the plastic distortion at the surface, is straightfor-ward: If we use a local coordinate system such that the x direction corresponds tothe profile direction and the y direction is normal to the average direction of thedeformed surface, then for small deformations the derivative yx ! @y=@x of theprofile y(x) is related to the component /pyx of the plastic strain tensor by

@y=@x ! /pyx#r$ % h/pyxi !: %/pyx#r$: #27$

By looking at an appropriately oriented surface and under single-slip conditions,this can be directly translated into the shear strain fluctuation %!.

Correlations in the plastic strain pattern can therefore be detected by surfaceprofile analysis. In particular, if the strain fluctuations %/pyx#r$ exhibit power-lawcorrelations this may lead to the emergence of self-a!ne surface profiles withroughness exponent * > 0:5 [8], as discussed below.

Self-a!ne surface morphology Several recent investigations have been devoted toself-a!ne scaling of the surfaces of plastically deformed metals. Zaiser et al. [8]applied a combination of atomic force microscopy (AFM) and scanning white-lightinterferometry (SWLI) to quantitatively characterize the surface of Cu polycrystalsover a range of scales between 10 nm and 2mm. Cu polycrystals of 99.9% nominalpurity were plastically deformed at room temperature, and two-dimensional surfacemaps were determined at various degrees of deformation up to an engineering strainof 23% (tensile stress 215MPa). The sequence of surface investigations was endedat the onset of macroscopic deformation localization (necking).

Multiple one-dimensional profiles were obtained from the surface maps in thedirections both parallel and normal to the tensile axis. Two typical AFM and SWLIprofiles are shown in figure 8. Roughness exponents were obtained by plotting meanheight di"erences hjy#x$ % y#x" L$ji vs. the separation distance L as shown infigure 9. Typical double-logarithmic plots exhibit linear scaling regimes extendingbetween 0.05 and 5 mm for the AFM and between 0.5 and 50 mm for the SWLIprofiles. The upper end of the SWLI scaling regime (the upper correlation length)was found to be strain-independent; it coincides with the mean grain size of thepolycrystalline aggregate. Roughness exponents deduced from the slope of the scal-ing regimes were similar for AFM and SWLI profiles, indicating continuous scalingover almost four orders of magnitude. The exponents were checked by also applyinga wavelet analysis method proposed by Simonsen et al. [51] to the surface profiles.Both techniques revealed a roughness exponent decreasing from an initial value closeto unity, during a strain interval of about 5%, towards an asymptotic value of* - 0:75. Surface profiles taken in the directions normal and parallel to the tensileaxis were found to yield similar exponents.

Self-a!ne scaling of deformed polycrystal surfaces is also evident from theprobability distributions of surface height di"erences. Distributions pL#$y$ of heightdi"erences $y :! y#x$ % y#x" L$ can be collapsed by re-scaling pL#$y$ !pL0 ##L=L0$*$y$ with a roughness exponent * - 0:75 (figure 10).

Scale invariance in plastic flow of crystalline solids 205

Downloaded By: [Karlsruher Inst fur Technologie Kit] At: 14:00 9 December 2010

The evolution of self-a!ne surface roughness was also studied on KCl singlecrystals deformed in compression [52]. Alkali halides o"er the advantage that verysmooth initial surfaces can be produced by cleavage. Deformation experimentson [100]-oriented crystals revealed a typical three-stage hardening curve wheredeformation at small strains (Stage I) proceeds in single slip with a comparativelylow hardening rate, whereas at higher strains multiple slip systems become activeand the strain hardening coe!cient increases (Stage II, see figure 11). Surfacecharacterization was done throughout these two hardening regimes using SWLI.Profiles taken in Stage I (figure 12, left), did not show any limits to the scaling regimebelow the profile length of 1.5mm. The roughness exponent * - 0:65determined from the profiles is somewhat lower than what is observed in polycrystalsand does not depend appreciably on strain. Roughness exponents *q were also

10005000 1500 2000$3

$2

$1

0

1

2

3

surf

ace

heig

ht y

[µm

]

position along surface x [µm]

$100

$50

0

50

1001050 15 20 25

position along surface x [µm]

surf

ace

heig

ht y

[nm

]

Figure 8. Surface profiles of a Cu polycrystal taken at / ! 9:6%; top: AFM profile; bottom:SWLI profile; the x direction is parallel to the direction of the tensile axis; roughness plotscorresponding to these profiles are shown in figure 9.

206 M. Zaiser

Downloaded By: [Karlsruher Inst fur Technologie Kit] At: 14:00 9 December 2010

determined from higher-order correlation functions scaling like hjh#x$ % h#x"L$jqi1=q / L*q . As expected for self-a!ne scaling, exponents *q, 1 0 q 0 4, werefound to be approximately independent of the order q of the correlation function.

In Stage II, on the other hand (figure 12, right), the profiles have a more complexstructure with a local roughness exponent * - 0:7 on small scales which on largerscales possibly crosses over to an exponent of about * - 0:5. At the same time, theroughening of the surface accelerates markedly (open data points in figure 11).

0.01 0.1 1 10 100 100010$2

10$2

100

101

102

103

104

(=1.0

3a2a

1a

3b2b1b(=0.8

1a ) = 0 AFM1b ) = 0 SWLI2a ) = 9.6%, AFM2b ) = 9.6%, SWLI3a ) = 17.8%, AFM3b ) = 17.8%, SWLI

<|y(

x)-y

(x+L

)|> [n

m]

displacement along surface L [µm]

Figure 9. Roughness plots (mean height di"erence vs. distance along profile) for AFM andSWLI profiles obtained from the as-polished surface and after deformation to strains of9.6 and 17.8%; the profiles for / ! 9:6% are shown in figure 8.

$3 $2 $1 0 1 2 30

20

40

60

80

100

L = 0.5 µm

L = 2.0 µm

L = 8.0 µm

L = 32.0 µm

cum

ulat

ive

prob

abili

ty [%

]

(L/L0)0.72'yL/y0

$4 $2 0 2 4

1

10

4070

95

99.5

prob

abili

ty[%

]

'yL/<'yL2>1/2

Figure 10. Scaling collapse of height di"erence distributions obtained from AFM and SWLIprofiles of Cu polycrystal surfaces (/ ! 9:6%); insert: distributions normalized to unit variancefor L ! 40 nm (dashed line), L ! 5 mm (full line) and L ! 160 mm (dotted line).

Scale invariance in plastic flow of crystalline solids 207

Downloaded By: [Karlsruher Inst fur Technologie Kit] At: 14:00 9 December 2010

The self-a!ne scaling of surface profiles y(x) observed in Cu polycrystals andafter Stage I-deformation of KCl single crystals implies that the underlying stochas-tic process %/pyx ! @y=@x% h@y=@xi has long-range spatial correlations along thedirection of the profile:

%/pyx#x$%/pyx#x0$% &

/ x% x0'' ''2*%2- x% x0

'' ''%0:3...%0:6: #28$

0.0

0.5

1.0

1.5

2.0

2.5

3.0

0 1 2 3 4 5 6 7 80

2

4

6

8

10

12

Str

ess

[MP

a]

rms

roug

hnes

s [µ

m]

strain [%]

Stage I Stage II

Figure 11. Stress–strain curve and rms surface roughness of a KCl single crystal deformed incompression at room temperature in [100] orientation; full line: stress–strain curve (compres-sive stress vs. engineering strain), open circles: rms surface roughness as determined fromfour profiles with length 1.5mm.

10$3 10$2 10$1 10010$4

10$3

10$2

10$1

100

101

10$4 10$3 10$2 10$1 10010$4

10$3

10$2

10$1

100

101

( = 0.5

( = 0.7

distance along profile [mm]

mea

n he

ight

diff

eren

ce [µ

m]

( = 0.65

mea

n he

ight

diff

eren

ce [µ

m]

distance along profile [mm]

Figure 12. Local roughening of the surface of a KCl single crystal as determined by SWLI(mean height di"erence vs. distance along profile); left: deformation in Stage I; strains 0%,0.56%, 1.16%, 1.44%, 2.01% and 2.67%; right: deformation in Stage II; strains 3.45%, 5.00%and 7.12%.

208 M. Zaiser

Downloaded By: [Karlsruher Inst fur Technologie Kit] At: 14:00 9 December 2010

Provided that the plastic strain itself has the characteristics of a point process (i.e. ifit is comprised of discrete and localized events), this power-law decay of the correla-tion function implies a correlation dimension of D - 0:5 for the distribution of suchevents along the line of the profile, and of D - 2:5 in three-dimensional space. Thisappears to be in line with the observations of Kleiser and Bocek on slip-line patterns,and with those of Weiss and Marsan on the spatial distribution of slip events [7, 48].

Dynamics of surface roughening In a large class of problems including the thermalroughening of elastic manifolds, the dynamic roughening of an elastic interfacedriven through a random medium, and diverse models of surface growth, the rough-ening dynamics can be described by the Family–Vicsek scaling, equation (17). In thiscase, roughening starts locally, over domains of size ' / t1=z where z is the dynamicexponent. The correlation length ' grows in time until it hits the system size, whereasthe magnitude of the roughness on scales below the correlation length remainsconstant in time.

The existing investigations of deformed single- and polycrystal surfaces, how-ever, indicate a di"erent growth kinetics, which may be more appropriately describedby the concept of anomalous scaling [53, 54]. For anomalous scaling, the localroughening is described by

y#x$ % y#x" L$'' ''% &

! t%L*loc fyL

t#1=z$

( ), #29$

and the global roughness of the surface grows like t*=z where *, *loc, and % are relatedthrough % ! #* % *loc$=z.

In their investigations on Cu polycrystals, Zaiser et al. found the self-a!nescaling regime to be delimited by a strain-independent upper correlation length ofthe order of magnitude of the grain size, indicating that the correlation length maybe an intrinsic material property (the grain size) rather than being governed by thedynamics of the roughening process. This idea was corroborated by Wouters et al.[55] who used confocal microscopy to investigate the surface morphology of poly-crystalline Al-Mg alloys of di"erent grain size. On scales below the grain size, theyobserve self-a!ne scaling with Hurst exponents * / 0:85–0.9 slightly above thosereported by Zaiser et al., whereas above this scale they find a scale-independent valueof the rms surface roughness. In the framework of anomalous scaling, equation (29),this can be formally expressed by setting z!1 while keeping % finite.

From the data of Wouters et al. [55], one deduces a growth exponent % - 0:8(figure 13). Curves pertaining to di"erent grain sizes LG can be collapsed byre-scaling the surface height in proportion with LG (insert in figure 13).Measurements on KCl single crystals reveal during Stage I a similar growthexponent % - 0:8, whereas during Stage II the growth exponent is somewhat larger(% - 1–1.5).

2.3. Deformation of micron-size samples

The heterogeneous and intermittent nature of plastic flow on microscopic and meso-scopic scales is not readily apparent in deformation experiments on macroscopiccrystals where, on scales above the fluctuation correlation length, the incoherentsuperposition of deformation events from di"erent parts of the specimen leads to

Scale invariance in plastic flow of crystalline solids 209

Downloaded By: [Karlsruher Inst fur Technologie Kit] At: 14:00 9 December 2010

a more or less smooth stress vs. strain, or strain rate vs. time, signals. Because of this,the avalanche-like character of deformation on smaller scales is not usually evidentfrom the recordings of standard tensile or compressive tests.

Recently, however, advances in machining have allowed Dimiduk andco-workers to prepare compressive specimens with diameters down to about 1 mm(for a discussion of specimen preparation methodology, see [56]). They performedcompression tests on ultra-small monocrystalline specimens of pure Ni [57–59] aswell as Ni-base superalloys [56, 57] and the Ni3Al intermetallic. Testing was carriedout in a standard nanoindentation system with a flat indentation tip acting as acompression platen. Compression was performed in a particular type of load con-trol, where the load is increased as long as the total (elastic " plastic) deformation ofthe specimen falls below a target value which increases linearly in time, and is keptconstant otherwise. This driving mode makes it possible to directly observe large slipavalanches, which in a displacement-controlled test would be stopped by the loaddrop that goes along with a sudden increase in strain. From a theoretical point ofview, it may be noted that this loading mode closely resembles the ‘quasi-staticdriving’ often applied in cellular automaton simulations of systems with intermittentavalanche dynamics (for examples, see sections 3.1 and 3.2): the load applied to thesystem is slowly increased as long as the activity of the system is zero, and is heldconstant during an avalanche. Stress vs. time and displacement vs. time curvesresulting from such tests are shown in figure 14. It is seen that the displacement(i.e. the plastic strain) increases in discrete steps; each strain step is followed bya stress plateau which lasts until the actual strain of the specimen is matched bythe ‘target strain’ which increases linearly in time.

In microtesting experiments carried out on specimens initially oriented for singleslip, deformation was found to proceed in simple shear on a single active slip system

1 100.1

1

10

1 100.1

1

rms

roug

hnes

s [µ

m]

strain [%]

*=0.8

scal

ed r

ough

ness

strain

Figure 13. Anomalous surface roughening of polycrystalline Al-Mg, grain sizesLG ! 90:1 mm (squares), 68.1mm (circles), 44.9mm (up triangles), 30.8 mm (down triangles);insert: scaling collapse obtained by scaling the surface width in proportion with LG; afterWouters et al. [55].

210 M. Zaiser

Downloaded By: [Karlsruher Inst fur Technologie Kit] At: 14:00 9 December 2010

up to comparatively large strains (! > 15%), leading to an extended Stage-Ibehaviour. At the same time, the deformation characteristics di"er dramaticallyfrom those of bulk samples:

. Intermittency of plastic deformation becomes evident as plastic flow proceedsin irregular bursts separated by quasi-elastic loading intervals. During thedeformation bursts, the plastic strain rate increases from near zero to verylarge values.

5 nm/sprogrammeddisplacement

rate

0

500

1000

1500

2000

2500

0

10

20

30

40

50

60

70

0 100 200 300 400 500 600 700 800

20 µm #4 (Ni_3)

Axial Displacement

Engineering Stress

Dis

plac

emen

t (nm

)E

ngineering Stress (M

Pa)

Time (s)

0

800

1600

2400

3200

4000

4800

5600

6400

0

50

100

150

200

250

300

0 200 400 600 800 1000 1200

30 µm #2 Ni3Al

DisplacementAxial Stress

Dis

plac

emen

t (nm

)E

ngineering Stress (M

Pa)

Time (s)

5 nm/sprogrammed

loadingrate

Figure 14. Compressive deformation of microsamples of pure Ni (top) and Ni3Al (bottom);shown are stress vs. time and displacement vs. time curves as recorded in microtestingexperiments (for details see text). Courtesy of D. Dimiduk.

Scale invariance in plastic flow of crystalline solids 211

Downloaded By: [Karlsruher Inst fur Technologie Kit] At: 14:00 9 December 2010

. As the stress is kept constant during each deformation burst, the stress–straincurves assume a shape reminiscent of a random ‘devil’s staircase’ with anirregular sequence of steps of widely varying magnitude. We note that a similarstep-wise increase of deformation with increasing stress may be observedin bulk samples on a local level, e.g. by monitoring the growth of slip bands[49, 60].

. The flow stress of small samples is larger than that of bulk specimens andincreases as the specimen dimensions decrease. This size e"ect cannot beattributed to the presence of strain gradients and ‘geometrically necessary’dislocations, which have become a commonplace explanation for size e"ectsin plasticity (for an overview, see, e.g. [61]): Owing to the single-slip simple-shear geometry, no geometrically necessary dislocations accumulate in thedeformation experiments under consideration. One has therefore to look forstatistical explanations of the observed size e"ect.

. The burst-like character of deformation becomes more evident as the specimendimensions decrease. At the same time, the stochastic nature of the flowprocess leads to increasing variations between deformation curves of di"erentspecimens, even if these have been machined out of the same single crystaland therefore share a common processing history.

The ‘devil’s staircase’ nature of the stress–strain curves obtained from micron-sized samples is confirmed by statistical analysis. This reveals a scale-free distributionof step sizes (strain increments $!) with an exponent ,! - 1:5–1.6 [59]. The scalingregime is limited to about two orders of magnitude in step size, since smaller eventsare obliterated by the mechanical noise of the experimental setup, but above thenoise threshold the power-law scaling is very convincing. Since plastic deformationis almost completely dissipative, the strain increment during a strain burst can bedirectly translated into the dissipated energy by multiplying it with the stress,$E ! "$!Vs where Vs is the specimen volume. Neglecting the (small) stress increasedue to hardening, we may therefore compare the exponent of the strain incrementdistribution observed by Dimiduk et al. and the energy exponent observed in AErecordings from deforming ice and hcp metals. This works out very well, as bothexponents are between 1.5 and 1.6, indicating that both distributions may begoverned by the same underlying physical processes.

3. Theoretical approaches

Di"erent theoretical approaches have been used for investigating collective phenom-ena in plastic flow on microscopic and mesoscopic scales. These approaches di"er inthe way the deformation state is represented; however, as we shall see, the mainresults obtained from di"erent approaches fit themselves into a consistent picture ofplastic yielding as a non-equilibrium phase transition. In the following we shalldiscuss (i) models which describe plastic flow in terms of the motion of discretelattice dislocations (dislocation dynamics); (ii) phenomenological models whichdescribe plastic deformation in terms of the evolution of shear strain oncrystallographic slip systems, and account for the influence of the underlyingdislocation dynamics in terms of fluctuations in the local stress–strain relationship

212 M. Zaiser

Downloaded By: [Karlsruher Inst fur Technologie Kit] At: 14:00 9 December 2010

(stochastic continuum models); (iii) phase-field models which take an intermediateposition as they describe plasticity in terms of shear strain on crystallographic slipsystems, but resolve the strain on a scale where individual dislocations can beidentified as localized gradients of the strain field. Each of these models can beused to describe heterogeneity and avalanche phenomena in plastic flow, and theavailable results appear to be mutually consistent.

3.1. Dislocation dynamics

The most straightforward approach towards modelling plastic flow in crystallinesolids on microscopic and mesoscopic scales is to investigate the stress-driven motionof interacting lattice dislocations. Individual dislocations or linear dislocation arraysinteracting with randomly distributed obstacles may be treated within the generalframework of elastic manifold depinning (see the introduction). In particular, it hasbeen shown by Moretti and co-workers [27] that planar arrays of dislocations of thesame sign (pile-ups or small-angle grain boundaries) exhibit long-range elasticity,with an elastic kernel #P which in Fourier space scales in proportion with themodulus of the wavevector, #P / jkj for jkj ! 0. This implies that the motion ofsuch arrays, depending on whether one is considering rigid or flexible dislocations,according to the terminology introduced in section 1.2 is in the class a ! d ! 1,or a ! 1, d ! 2. Simulations of the motion of a one-dimensional array of rigiddislocations through a pinning field reported by Moretti et al. indeed showexponents similar to those given for the a ! d ! 1 case in table 1. Interestingly,this seems to be true irrespective of whether the dislocations are arranged in anarray perpendicular to their direction of motion (a grain boundary), or form aprocession on the same slip plane (a pile-up) – even though in the latter case long-range correlations are present in the disorder as the dislocations move one afteranother through the same pinning field. For the physically realistic case of a planararray of flexible dislocations (a ! 1, d ! 2) one expects mean-field behaviour.Observations of the dynamics of such arrays via slip-line kinematography areconsistent with this expectation (section 2.2.2).

For the dynamics of more general dislocation systems consisting of dislocationsof di"erent signs and/or moving on di"erent slip systems, the depinning frameworkcannot be directly applied. One therefore has to rely on numerical simulations(section 3.1) for investigating the dynamic evolution of such systems underexternally applied loads.

3.1.1. Simulation methods. Two-dimensional (2D) dislocation dynamics idealizesthe dislocation system as a system of straight parallel lines. The simulations thereforeessentially correspond to molecular dynamics simulations of particles moving in aplane. Three-dimensional (3D) dislocation dynamics, on the other hand, simulatesthe evolution of a system of flexible and reactive lines in three spatial dimensions.Both approaches have to cope with the fact that the dislocations are endowedwith long-range #1=r$ stress fields which cannot easily be truncated, and that thesimulations therefore tend to be computationally expensive.

2D dislocation dynamics Two-dimensional dislocation dynamics is conceptuallysimple: Dislocations are envisaged as charged point particles in a plane.

Scale invariance in plastic flow of crystalline solids 213

Downloaded By: [Karlsruher Inst fur Technologie Kit] At: 14:00 9 December 2010

Their motion is driven by the stress applied from outside to the deforming body, andthey interact through long-range stress fields. If dislocation climb is neglected, themotion of these ‘dislocation particles’ is confined to the lines of intersection betweenthe slip planes of the respective crystallographic slip systems and the simulation plane.

In most dislocation dynamics simulations, dislocation motion is assumed tooccur in an over-damped manner. If dislocation glide is governed by electron andphonon drag forces, this leads to a linear relationship between the Peach–Koehlerforce FPK in the glide plane, and the dislocation glide velocity. The glide componentof the Peach–Koehler force can be written as [cf. equation (8)]

FPK#r$ ! egsb"#r$: #30$

Here eg is a unit vector pointing in the dislocation glide direction, the product sb ofthe sign s ! eg)t* n+ of the dislocation and the modulus b of its Burgers vector canbe interpreted as the ‘charge’ of the 2D point particle representing the dislocation,and "#r$ is the local resolved shear stress in the dislocation slip system. Assuming alinear force–velocity relationship and considering dislocations of a single slip systemonly, one gets the system of equations

$@txi ! si " "X

k6!i

sk"D#ri % rk$" #

, #31$

where $ is the dislocation drag coe!cient, the slip direction has been chosen to bethe x direction, " is the externally applied shear stress, and "D#r$ is the stress field ofan individual dislocation. For an edge dislocation (b ! bex) one has

"#r$ ! Gb

2p#1% +$x x2 % y2+ ,

r2+ ,2 : #32$

where + is the Poisson number of the material. The local shear strain rate createdby the dislocation system is

_!#r$ ! bX

k

sk@txk%#r% rk$: #33$

Simulations assuming a linear relationship between stress and dislocationvelocity are very common both for 2D and 3D dislocation systems. However, it isimportant to note that experimental results on dislocation velocities show a muchmore complicated picture. As discussed in detail in the overview by Nadgorny [62],the dislocation velocity increases linearly with stress only in the high-stress regime,whereas at low stresses a strongly nonlinear (exponential) stress dependence isobserved. For the dynamics of dislocation systems this is important, since at nottoo high applied stresses the motion of dislocations is strongly intermittent: Thedislocations spend most of the time in low-stress configurations, which thereforecontrol the mean velocity, and experience high stresses only during intermittentjumps between such configurations. The popularity of linear stress–velocity relation-ships has much to do with the fact that strongly nonlinear relationships increase thenumerical sti"ness of the simulations and may easily render their computational costprohibitive. However, an easy and computationally e!cient expedient for mimickingthe e"ect of a strongly linear stress–velocity relationship is to use extremal dynamics

214 M. Zaiser

Downloaded By: [Karlsruher Inst fur Technologie Kit] At: 14:00 9 December 2010

or automaton models where the dislocation moves (on the time scale considered)instantaneously to the next stable position whenever the stress exceeds a giventhreshold, and remains stationary otherwise. Results from such simulations will bediscussed in the following, and compared to those obtained from simulations whichassume linear stress–velocity laws.

Another important issue in 2D dislocation dynamics concerns the problem ofdislocation multiplication. In deforming crystals, the total dislocation density (linelength per unit volume) usually increases with increasing deformation, since theexpansion of curved dislocation loops goes along with an increase in line length.Such ‘dislocation multiplication’ is important for two reasons: (i) In crystals withvery low initial dislocation density, the proliferation of dislocations at the onset ofdeformation may lead to a transient softening. (ii) At larger dislocation densities, onthe other hand, increasing the dislocation density increases the amplitude of thefluctuating internal-stress field in the deforming crystal and the strength of config-urations in which dislocations mutually trap each other. The flow stress thenincreases according to the Taylor relationship, equation (34): the system exhibitsstrain hardening. Since loop expansion cannot occur in a system of straight lines,there is no straightforward method to account for dislocation multiplication in 2Ddislocation dynamics. Researchers have tried to solve the problem by definingdi"erent kinds of phenomenological rules for introducing new dislocations intothe system. However, as dislocations carry long-range stress fields, the creation ofa new dislocation may discontinuously change the stress everywhere in the system,and thereby introduce all kinds of artefacts into the dynamics. To remedy thisproblem, several things can be done: (i) Dislocations should be introduced in pairsof opposite sign, since dislocation multiplication must conserve the total Burgersvector of the dislocation system. (ii) By placing the dislocations of such a pair closeto each other, the stress discontinuity can be reduced. (If they are placed too close,however, because of their strong mutual attraction they will never become separated,and therefore contribute little to the dynamics.) (iii) By using di"erent phenomen-ological rules, and comparing the outcomes, one may try to ensure that the results ofa simulation do not depend crucially on the details of the dislocation multiplicationrule.

A similar but less serious problem occurs if dislocations of opposite sign areallowed to instantaneously annihilate if their spacing falls below a certain cut-o"distance. Computationally this is a ready expedient for reducing the computationalsti"ness of the simulations, since one avoids integrating the dynamics ofconfigurations with large interaction forces. It is also physically less problematicthan introducing dislocation multiplication since: (i) the total Burgers vector isconserved by definition in this process; (ii) the stress discontinuity due to theannihilation is small since the dislocations are close anyway; and (iii) the processis physically motivated, since straight edge dislocations of opposite sign have beenobserved experimentally to annihilate below distances of about 4b [63].

Another issue concerns initial and boundary conditions. In most simulationsdiscussed in the following, periodic boundary conditions were imposed to mimicbulk behaviour. Initial conditions may be prescribed by distributing dislocationsor dislocation sources according to some given statistical rule. In doing so it isimportant to note that a completely uncorrelated, statistically random initial

Scale invariance in plastic flow of crystalline solids 215

Downloaded By: [Karlsruher Inst fur Technologie Kit] At: 14:00 9 December 2010

distribution of dislocations is unphysical since it implies an elastic energy densitywhich diverges logarithmically with the system size [64]. One way to circumvent thisproblem is to use an initially random distribution but then, before studying theplastic flow dynamics, carry out a relaxation step at zero applied stress until theelastic energy of the system has stabilized. The relaxation of an initially randomdislocation system is in itself an interesting, if somewhat academic, topic as it followsa slow dynamics governed by non-trivial power laws [65]. More interesting in viewof the explanation of experimental observations is the subsequent evolution of theplastic deformation rate under constant applied stress, both in view of thecreep behaviour and in view of the observation of intermittent avalanche-likedynamics (sections 3.1.2 and 3.1.3).

In most 2D dislocation dynamics simulations discussed in the following sections,the number of dislocations in a simulation has either been conserved, or a steadystate with low rates of multiplication and annihilation (i.e. an almost conserveddislocation number) was reached and the influence of di"erent rules for dislocationmultiplication has been tested. One may therefore expect that the results of thesesimulations represent generic features of the dynamics of interacting dislocationsand are not too heavily influenced by artefacts of the simulation technique.

3D dislocation dynamics Three-dimensional dislocation dynamics simulations is ascience of its own. For a detailed discussion of such simulations, the reader isreferred so some topical reviews [66, 67]. Problems similar to 2D are the long-range interactions between dislocation segments which cannot be truncated, andwhich in 3D make these simulations computationally very expensive. New problemsarise from the necessity to describe a system of flexible lines with non-conserved linelength, the need to maintain the connectivity of these lines, and the fact that twointersecting dislocations of di"erent slip systems may react to create segments ofa third slip system. For the scope of the present review, 3D dislocation dynamicssimulations are of limited interest since the computational cost associated with suchsimulations has until now precluded their application to systems that aresu!ciently large to detect long-range correlations and scale-free behaviour. Eventhough large systems have been studied in ‘one-o"’ simulations, a proper statisticalanalysis of scale-free fluctuation phenomena in plastic deformation which involvesthe simulation of a large ensemble of systems has not yet been attempted. It may beexpected that this situation will change in the near future, as the problem lends itselfto ‘trivial parallelization’ on multiple computers, and standard computers may soonbecome powerful enough to run 3D dislocation dynamics simulations of appreciablesize within acceptable time limits. At the same time, experimental observations cannow be made on scales that are directly accessible to 3D simulation (see section 2.3on micron-sized samples), allowing for a direct experimental validation of simulationresults.

Scaling relations for dislocation systems Before discussing simulation results, it isuseful to recall some general scaling relations which apply if the motion of disloca-tions is mainly controlled by their mutual interactions, rather than by lattice e"ects(Peierls stress) or by interactions with atomic defects or with precipitates. The stressfield created by a dislocation in 2D scales like 1=jrj, and that created by a dislocationsegment of length ds in 3D like ds=jrj2. We now consider a dislocation arrangement

216 M. Zaiser

Downloaded By: [Karlsruher Inst fur Technologie Kit] At: 14:00 9 December 2010

which is in (metastable) equilibrium at some external stress " and decrease alldistances by a factor ). Since the dislocation density . is for a 2D dislocation systemdefined as the areal density of intersection points with a plane normal to thedislocation lines, and for a 3D dislocation system as the line length per unit volume,this operation in either case increases the dislocation density by a factor )2.Evidently, the new dislocation arrangement is in equilibrium at the stress )".

More generally speaking, if a dislocation arrangement of density . is inequilibrium at the stress ", then an otherwise statistically equivalent arrangementof density .0 is in equilibrium at the stress "#.0=.$1=2. The same argument appliesto loss of (meta)stability at some critical stress (yield stress) "c: the yield stress ofa dislocation arrangement scales in proportion with the square root of dislocationdensity, as expressed by Taylor’s relation

"c ! 0Gb---.

p: #34$

The scalar pre-factor 0 depends on the nature of the ‘yielding transition’. For a singledislocation interacting with the stress fields of dislocations with density . threadingits glide plane, yielding corresponds to the depinning transition of a weakly pinnedelastic line [17]; if the dislocation can react with the threading ‘forest dislocations’,these are much stronger obstacles, and yielding may correspond to invasion percola-tion [68]; if we have a 2D system of straight interacting dislocation lines, the onsetof plastic flow has been discussed in analogy with a jamming transition [69] (see nextsection). In either of these cases, the critical stresses for depinning/percolation/unjamming fulfil the Taylor relationship.

Some other scaling relations are also straightforward. Assuming that dislocationcreation and annihilation are not prominent, the shear strain can be understood asthe product of dislocation density and mean glide path, ! ! .bL. Consider nowa rearrangement in the dislocation system which produces a strain increment $!in a system of linear extension Ls and dislocation density .. Trivially, a similarrearrangement in a statistically equivalent system of size Ls=) and density )2. pro-duces a strain increment )$!, since the glide path decreases like .%1=2. We considernow the case where Ls is large enough such that boundary and finite-size e"ects arenot important, and omit the re-scaling of the system volume. In this case, for the slipevent $! in the system with density . there is still an equivalent event in the systemwith density )2.. Referring the strain increment to the entire system, this eventnow produces the total strain increment $!=)d%1 where d 2 f2, 3g is the systemdimension. The same scaling property holds for parameters such as the average,the median, or the ‘largest’ and ‘smallest’ events in an arbitrary event sizedistribution.

These scaling relations (often referred to as ‘laws of similitude’ in the metallur-gical literature [14]) may seem trivial, but they have important consequences. Theyallow to deduce the behaviour of dislocation systems of di"erent densities from asingle set of simulations by means of simple scaling transformations. We use this inthe simulations reported in sections 3.1.3 and 3.2.2 where we give lengths, stressesand strains in the respective ‘natural units’ .%1=2, Gb.1=2, and b.1=2. Finally we shalluse them, together with our simulation results, to obtain estimates of the magnitudeand observability of dislocation avalanches in macroscopic deformation experiments(section 4.1).

Scale invariance in plastic flow of crystalline solids 217

Downloaded By: [Karlsruher Inst fur Technologie Kit] At: 14:00 9 December 2010

3.1.2. Relaxation and creep of two-dimensional dislocation systems. Miguel et al.[69, 70] studied the creep relaxation of 2D dislocation systems consisting of equalnumbers of dislocations of a single slip system, assuming a linear stress–velocity law.Periodic boundary conditions were imposed for the stresses and dislocation motions,the dislocations were initially placed at random and the initial configuration wasrelaxed at zero internal stress. A constant shear stress was then applied and theevolution of the shear strain rate d!=dt /

Pi sivi was monitored.

While the creep dynamics in individual simulations is strongly intermittent andcharacterized by irregular bursts [70], after averaging over many individual simula-tions a coherent picture emerges: During a transient after application of the externalshear stress, the creep behaviour is characterized by power-law relaxation of thestrain rate, with a relaxation exponent close to 2/3 ( _! / t2=3, see figure 15).Accordingly, the creep strain increases in time as ! / t1=3. After the initial transient,the deformation behaviour bifurcates depending on the applied stress: Below acritical stress, the deformation rate relaxes exponentially towards zero (the systemgets jammed) whereas above the critical stress, the deformation rate becomes asymp-totically constant. Power-law relaxation regimes of appreciable length can be foundover a wide range of stresses. These findings compare well with Andrade’s oldobservation of a ‘universal’, i.e. material-independent ‘primary’ or transient creepregime [71, 72] during which the creep strain increases like ! / t1=3, and which isfollowed by a ‘secondary’ regime during which the creep rate is roughly constant.

Above the critical stress the system reaches an asymptotically constant creeprate. This statement is, however, correct only in the sense of a statistical averageover many systems. In an individual simulation, the strain rate undergoes largefluctuations, and it has been attempted to relate these fluctuations to the acousticemission bursts observed in ice single crystals that we have discussed in section 2.1.

100 101 102 103 104 10510$4

10$3

10$2

10$1

100

101

! = 0.025! = 0.075! = 0.100! = 0.125! = 0.175! = 0.225! = 0.325

stra

in r

ate

[arb

itrar

y un

its]

time [arbitrary units]

Figure 15. Strain rate relaxation of a 2D dislocation system for di"erent applied stresses;stresses in units of Gb

---.

p; the solid line is the best linear fit of the 1! 0.1 curve and yields

d!=dt / t%0:69. After Miguel et al. [69].

218 M. Zaiser

Downloaded By: [Karlsruher Inst fur Technologie Kit] At: 14:00 9 December 2010

Dislocation avalanches in creep deformation In several papers, Miguel et al.investigated the possibility of explaining experimentally observed AE signals interms of the intermittent bursts of dislocation activity observed in their creepdeformation simulations [5, 6]. In addition to the strain rate, they monitored thesum V !

Pi jvij of the absolute velocities of the dislocations. Since the friction

force in the overdamped dynamics was assumed proportional to velocity, V isproportional to the energy dissipated per unit time by the dislocation system.One observes an intermittent and burstlike V(t) signal on top of a continuousbackground. Provided that AE recordings provide a faithful representation ofthe dissipation characteristics of dislocation systems, it should be possible to relatethe statistics of the simulated dissipation bursts to those of the experimentallyobserved AE signals.

To eliminate the continuous background, Miguel et al. used two methods:In one paper [5], a simple thresholding procedure was used to split the V(t)signal into discrete bursts B, and the energy dissipated during a burst wasobtained as E /

*BV#t$dt. The cumulative energy distribution obtained in this

manner was observed to decay with an exponent ,E % 1 - 0:6, which is in goodagreement with the experimental observations discussed in section 2.1. In asecond paper [6], the procedure was slightly di"erent since only dislocationswith velocities above the velocity corresponding to the externally applied stresswere included in the evaluation of V. Since such ‘fast’ dislocations move in thedirection imposed by the applied stress (this is not true for ‘slow’ dislocations,as will be discussed below), the value of V evaluated with the velocity thresholdis in fact a proxy for their contribution to the overall strain rate. The acousticenergy was then defined as the square of V, which again lead to a power-lawdistribution with an exponent ,E - 1:8 which is in acceptable agreement withexperiment.

An interesting feature in the creep simulations of Miguel et al. is the presence oftwo physically distinct contributions to the strain and energy dissipation rates: (i) Amajor part of the dislocations at each moment is organized into slowly drifting multi-dislocation configurations (dipoles and multipoles). Dislocations of di"erent signsform clusters which drift slowly into one or the other direction, depending on theirnet Burgers vectors and on the presence of stress gradients. Dislocations trapped insuch clusters do not necessarily move in the direction imposed by the external stress.Since the clusters mostly have small net Burgers vectors, and their motion tends to beslow, they contribute little to the acoustic emission signal and even less to the strainrate. However, because of their large number such slowly moving dislocations stilldissipate an appreciable amount of energy. (ii) The strain rate and acoustic emissionsignals are governed by small numbers of dislocations which break free from theslowly moving configurations and move rapidly under the action of external andinternal stresses until they become trapped again. The rapid motion of onedislocation changes the stress everywhere in the system and may help otherdislocations to break free. This mechanism is at the core of the observed avalanchedynamics. However, a quantitative analysis of the avalanche motion is complicatedby the fact that the distinction between ‘slow’ and ‘fast’ dislocations requires theintroduction of some artificial threshold. That such a threshold is somewhatarbitrary can be seen from the fact that the distribution p(v) of the dislocation

Scale invariance in plastic flow of crystalline solids 219

Downloaded By: [Karlsruher Inst fur Technologie Kit] At: 14:00 9 December 2010

velocities itself exhibits a power-law scaling regime, p#v$ / v%2:5 [6]. (Interestingly,this simulation result has received direct experimental confirmation in a recentinvestigation of Pertsinidis and Ling [73], who monitored the motion of edgedislocations during shear deformation of colloidal crystals.)

The problem of slowly moving dislocation configurations results partlyfrom the assumption of a linear relationship between stress and dislocationvelocity. Experimental investigations (for an overview, see the work ofNadgorny [62]) demonstrate that the velocity of dislocations is a linear functionof stress only in the regime of high stresses, whereas at low stresses the velocityis governed by the interaction of dislocations with atomic defects, or with thePeierls potential of the crystal lattice, and therefore becomes a strongly nonlinear(exponential) function of the locally acting stress. This implies that multipoleconfigurations, in which each dislocation experiences only a quite small stress,may be e"ectively immobile on the time scale of the experiment. Dislocationdynamics simulations with strongly nonlinear stress–velocity laws are computa-tionally inconvenient, but the qualitative e"ect of a strong nonlinearity in thestress–velocity relationship can be easily assessed by using models with extremaldynamics (only the dislocation with the largest stress is allowed to move) orautomaton models (dislocations move with unit velocity once the stress exceedsa threshold value). The results of such simulations indicate that the avalanchedynamics remains more or less unchanged, whereas the slowly moving configura-tions become ‘frozen’ and transform into e"ectively immobile trappingconfigurations [74].

3.1.3. Stepwise deformation curves and critical behaviour at yield. In a creep testthe external stress is kept constant and the strain rate signal is recorded. Duringusual tension or compression tests, on the other hand, the applied stress is slowlyincreased from zero, and the stress–strain curve is recorded. There is a distinctionbetween deformation-controlled tests where the stress is increased such as to main-tain a given imposed deformation rate, and the stress is recorded as a function oftime (strain), and stress-controlled tests where a constant stress rate is imposed andthe strain is recorded. The distinction is, however, immaterial if one considers thedeformation of a small volume embedded into a macroscopic crystal; in this case thelocal conditions always correspond to those in a stress-controlled test since localfluctuations of the deformation rate do not a"ect the stress applied from outside tothe macroscopic deforming body.

The behaviour of dislocation systems during stress-controlled deformationtesting was investigated by Zaiser et al. [74]. As in the simulations of Miguel andco-workers, deformation on a single slip system with equal numbers of positiveand negative dislocations was considered and periodic boundary conditions wereimposed. Also similar was the choice of initially random dislocation positions andsubsequent relaxation of the dislocation system before an external stress was applied.However, an automaton technique was used for the dynamics: Dislocations weremoved simultaneously on a discrete grid according to the sign of the locally actingstress, conditional on the requirement that the sign of the stress experienced bya given dislocation did not change during a move. The external stress was increasedadiabatically slowly, i.e. an external stress increment was applied only after all

220 M. Zaiser

Downloaded By: [Karlsruher Inst fur Technologie Kit] At: 14:00 9 December 2010

dislocation activity had ceased. Alternatively, an extremal dynamics was used where

only the dislocation with the largest stress was moved at a time, thus mimicking a

strongly nonlinear stress–velocity relationship where all dislocations are practically

at rest on the time scale of the fastest moving one. The dislocation number was

conserved, i.e. neither dislocation multiplication nor annihilation were taken into

account.Stress–strain characteristics were determined by simultaneously recording the

stress and the total strain ! ! #b=L2s $P

i siLi, where L2s is the simulated area, si

is the sign of the ith dislocation and Li ! xi % xi, 0 is its (if necessary periodically

continued) glide path. Simulations were terminated at a prescribed maximum strain.

Results are shown in figure 16 where stress and strain are given in the respective

‘natural units’ for a dislocation system (cf. our discussion of scaling relations above).

It is seen that the stress–strain curves assume a staircase-like shape similar to the

experimental curves of micron-sized specimens discussed in section 2.3. Also in

agreement with the experimental observations reported in that section is the fact

that there is substantial scatter between di"erent simulations. This scatter does not

represent any di"erences in the material properties but simply reflects the outcome

of di"erent initial positions of the dislocations. Only after averaging over many

simulations, can a smooth stress–strain characteristics be obtained, and it becomes

evident that the strain diverges logarithmically as the stress approaches a critical

value "c (yield stress, see insert of figure 16). The logarithmic divergence corresponds

to a horizontal asymptote in the stress vs. strain graph, i.e. the model does not

0 4 8 12 16 200.0

0.1

0.2

0.3

0.4

shea

r st

ress

[Gbr

1/2 ]

shear strain [br1/2]

0.01 0.1 10

10

20

30

stra

in[b

r1/2 ]

!C-!

Figure 16. Stress–strain curves in simulated stress-controlled tests on systems of size32* 32 . (1024 dislocations); insert: average stress–strain behaviour obtained by averagingover 100 simulations.

Scale invariance in plastic flow of crystalline solids 221

Downloaded By: [Karlsruher Inst fur Technologie Kit] At: 14:00 9 December 2010

display hardening. (This is to be expected, since no dislocation multiplicationmechanism was introduced.)

The statistical distribution of critical stresses obtained from di"erent simulationsof statistically equivalent systems depends on system size. This is illustrated infigure 17 which shows probability distributions of yield stresses obtained fromensembles of systems of area L2

s ! 8* 8=. to L2s ! 64* 64=. corresponding, for a

typical dislocation density of . ! 1012 m%1, to sizes of 8* 8 to 64* 64 (mm2). It isseen that the width of the distributions increases with decreasing system size,indicating an increasing scatter in the deformation behaviour. At the same time,the average yield stress increases for smaller systems. It is important to note thatthis size e"ect in the simulations is of a purely statistical nature and does not relate tosurface e"ects or e"ects of dislocation sources, as periodic boundary conditions wereused and a conserved number of dislocations was assumed. Both the increasingscatter and the increase in strength with decreasing system size match the observa-tions in deformation of micron-sized specimens reported by Dimiduk et al. [57, 58],although the magnitude of the size e"ect is underestimated.

The behaviour in the individual simulations is characterized by large steps in thestress–strain curves (dislocation avalanches). The statistics of these avalanches hasbeen investigated as a function of stress. Avalanches were characterized in terms ofthe total slip length increment Lav !

Pi si$Li where $Li is the di"erence between

the positions of the ith dislocation before and after the avalanche. This makes itpossible to directly compare simulations of systems of di"erent area – the total strainincrement $! ! bLav=L

2s , on the other hand, is inversely proportional to the simu-

lated area L2s . Avalanche size distributions p"#Lav$ were determined over narrow

stress intervals centred around di"erent stresses ". Results are shown in figure 18for $ ! #1% "="c$ ! 0:2, . . . , 0:8.

One observes power-law distributions of dislocation avalanche sizes witha common exponent , - 1:4. Whereas this exponent does not depend on stress,

0.2 0.3 0.4 0.5 0.6

0.0

0.2

0.4

0.6

0.8

1.0

8+8, 100 systems161+16, 100 systems32+32, 150 systems64+64, 27 systems

prob

abili

ty P

(!C

<!)

stress ! [Gbr1/2]

Figure 17. Distributions of yield stresses obtained for systems of di"erent sizes (system sizein units of 1=

---.

p).

222 M. Zaiser

Downloaded By: [Karlsruher Inst fur Technologie Kit] At: 14:00 9 December 2010

the maximum avalanche size increases like #1% "="c$%1=1 with 1 - 0:5 as the stressapproaches the yield stress. Accordingly, distributions pertaining to di"erent stresslevels obey the scaling form

p"#Lav$ ! L%,av fL

Lav

$1=1

( ): #35$

These distributions can therefore be collapsed by re-scaling Lav ! Lav$1=1 (figure 18,

right). It is also seen that power-law scaling is quite robust as scaling over more thanthree decades persists even at stresses that are just one fifth of the critical stress. Thisobservation of robust scaling behaviour quite far from a critical point has also beenmade in other systems exhibiting avalanche dynamics [75].

In our model, the work Vs"$! which is done by the external stress " duringan avalanche is completely dissipated. The proportionality between the energydissipation and the strain increment (or equivalently the total slip length coveredby dislocations during an avalanche) suggests a comparison between the avalancheexponent , obtained from the present simulations and the energy exponent ,Eobserved in the statistics of AE bursts. With , - 1:4 and ,E ! 1:5–1.6 this compar-ison works out quite satisfactorily. The avalanche exponent , ! 1:4 also compareswell with the exponent ,! ! 1:5–1.6 of step size distributions from stress–straincurves of micron-sized samples [59].

At this point, we note that some caution is required when bursts fromdi"erent parts of the stress–strain curve are added up. To illustrate the problem,we consider the integral distribution of avalanche sizes along the stress–strain curveas obtained from our simulations. This integral distribution is related to the stress-dependent distributions (which correspond to small stress intervals centred around

10$1 100 101 102 103 104 10510$9

10$8

10$7

10$6

10$5

10$4

10$3

10$2

10$1

10$2 10$1 100 101 102 10310$8

10$7

10$6

10$5

10$4

10$3

10$2

10$1

100

prob

abili

ty d

ensi

ty p

(Lav

)

&=1.4

'=0.2'=0.4'=0.6'=0.8

total slip length Lav [r$1/2]

'=0.2'=0.4'=0.6'=0.8

prob

abili

ty d

ensi

ty p

(Lav

)/(1

-!/!

c)2

scaled slip length (1-!/!C)2Lav

Figure 18. Distributions of dislocation avalanche sizes measured in terms of the total slipdistance covered by dislocations during an avalanche; right: collapse of distributions obtainedfor di"erent sized if size is re-scaled by Lav ! Lav#1% "="c$2.

Scale invariance in plastic flow of crystalline solids 223

Downloaded By: [Karlsruher Inst fur Technologie Kit] At: 14:00 9 December 2010

specific stress levels) via

pint#Lav$ /"p"#Lav$d" / L%#,"1$

av : #36$

Each of the distributions p" has the same exponent , but a di"erent cut-o". Theintegral distribution pint, on the other hand, exhibits no cut-o" but a modifiedavalanche exponent ," 1 which by itself does not characterize the critical behaviour– rather, it combines two di"erent exponents characterizing (i) the scaling regimeof the avalanche size distribution and (ii) the scaling of its cut-o". This behaviourhas been explicitly demonstrated in [74]. Of course, our consideration applies to ahypothetical non-hardening material and real materials with finite hardeningcoe!cients may behave di"erently. Nevertheless it illustrates the dangers incurredwhen information is added up which pertains to di"erent states of the system(i.e. to di"erent separations from its critical point).

The behaviour of conserved two-dimensional dislocation systems withautomaton or extremal dynamics under slow loading can be summarized as follows:(i) The strain diverges logarithmically as the stress approaches a critical value (yieldstress). (ii) The response of the system to an increasing stress is characterized byan irregular sequence of strain bursts with power-law size distribution. (ii) This scale-free behaviour is manifest already at stresses well below the yield stress and persistsup to a maximum burst size which diverges at yield. (iii) The exponents characteriz-ing the critical behaviour (avalanche exponent , - 1:4, divergence of the maximumburst size like #" % "c$%2) have approximately the values expected for mean-fielddepinning (see the introduction), even though the main ingredients of depinningmodels (dynamics of an elastic manifold, quenched disorder) are absent in thesimulations.

To better understand the type of critical behaviour we are dealing with, it isuseful to look at an apparently quite di"erent class of models which operate on ascale where individual dislocations cannot be resolved and plastic deformationis described in terms of the evolution of a continuous plastic strain field.

3.2. Models of microstrain evolution

Dislocation dynamics directly traces the motion and collective dynamics of defectsduring plastic flow. Randomness, heterogeneity and stochastic behaviour indislocation dynamics models stem from the probabilistic choice of initial conditionsfor the otherwise deterministic evolution of a discrete dislocation system. Analternative approach towards modelling collective phenomena in plastic deformationconsists in the adaptation of continuum plasticity models to include microstructuralheterogeneity and randomness in a phenomenological manner.

3.2.1. Constitutive equations. As discussed in the introduction, continuummechanical constitutive equations connect the stress, plastic strain, and strain ratein a material. Such models operate on scales above the ‘microscopic’ scale whereindividual dislocations may be resolved. Accordingly, stress and strain must beconsidered as mesoscopic fields which are space dependent on a scale which isabove the dislocation spacing, but small in comparison with the macroscopic

224 M. Zaiser

Downloaded By: [Karlsruher Inst fur Technologie Kit] At: 14:00 9 December 2010

dimensions of the deforming body. Stresses associated with individual dislocationsare not resolved, but enter the formulation implicitly since dislocation interactionsdetermine the local yield stress of the material and its evolution with strain.

Deformation heterogeneities and internal stresses In the following we focus on thebulk behaviour of materials which are heterogeneous and random on microscopicand mesoscopic scales but homogeneous on the macroscopic scale. In this case theproblem of evaluating the stress state of the material can be split into two parts: (i)Tractions applied from outside to the surface of the deforming body, or displace-ments prescribed on the surface of that body, create an ‘external’ stress D which weconsider space-independent over the region of interest. (ii) Because of heterogeneitiesin the material properties, plastic deformation may in general proceed in a spatiallyheterogeneous manner on mesoscopic scales. Deformation heterogeneities give riseto eigenstresses Dint. (A special case of such eigenstresses are actually the stressesassociated with dislocations, where the heterogeneity corresponds to the boundaryof a slipped area.) Provided that surface e"ects can be disregarded over the regionof interest, the internal stress tensor can be written as a functional of the plasticstrain field,

Dint#r$ ! %!0 !p#r$ % h!pi# $

""!1#r% r0$!p#r0$d3r0, #37$

where h!pi is the average plastic strain. Explicit expressions for the Green’s functions!0 and !1#r$ have been given by Zaiser and Moretti for solids of arbitrary symmetry[76]. The special case of an incompressible isotropic material was considered byPicard et al. [77] where also the e"ect of boundaries was investigated.

In the following we consider the special case of an isotropic material deformingin plane strain on a single slip system. The slip planes are normal to the y axis, slipoccurs in the x direction, and the strain field is assumed to be independent of z. Thisis equivalent to the deformation geometry investigated by 2D dislocation dynamicsin the previous section. Plastic deformation is here completely characterized by theshear strain ! ! 2/pxy ! 2/pyx. The internal resolved shear stress in the considered slipsystem is given by [76, 78]

"int#r$ !G

2p#1% +$

"!#r0$ 1

#r% r0$2% 8#x% x0$2#y% y0$2

#r% r0$6

" #

d2r0

" G

4#1% +$)h!i% !#r$+, #38$

or, in Fourier space,

"int#k$ ! % G

p#1% +$!#k$

k2xk2y

jkj4: #39$

Regarding these expressions, two points may be noted: (i) The elastic kernel is notpositive definite in real space. (ii) Strain fluctuations with wavevectors parallel tothe x or y directions do not give rise to internal stresses. The implications will bediscussed below.

Scale invariance in plastic flow of crystalline solids 225

Downloaded By: [Karlsruher Inst fur Technologie Kit] At: 14:00 9 December 2010

Constitutive equations: viscoplastic flow of a random material To relate the stressto the evolution of the strain field !#r$, we adopt a linear viscoplastic constitutiverelation of the type discussed in the introduction. The evolution of the local shearstrain ! is given by [cf. equation (4)]

$@t! ! j" " "intj% "y#!,r2, r$+ ,

sign#" " "int$, j" " "intj > "y#!,r, r$,0 else:

(

#40$

Here " is the externally applied resolved shear stress, "int is the internal shear stressdue to deformation heterogeneities, and "y#!,r, r$ is the local yield stress.Randomness and heterogeneity in the material microstructure and microstructureevolution are taken into account in a phenomenological manner by allowing for astochastic dependence of the yield stress on space and strain. Furthermore, internallength scales associated with the material microstructure can be taken into accountby allowing the yield stress to depend on the second gradient of strain [12, 78].

In plastically deforming crystals, the local yield stress reflects the fine-scaledynamics of the interacting dislocations on scales below the spatial resolution ofthe mesoscopic model. For this case, Zaiser and co-workers [76, 78] proposed torelate "y to the fluctuating internal stress field created by the dislocations in thedeforming crystal. This led to the following constitutive relation for the deformationresistance:

"y#!,r, r$ ! %C@2!

@x2" %"#r, !$: #41$

The fluctuating stress %"#r, !$ is associated with the ‘microscopic’ stress field createdby individual dislocations. For a two-dimensional system of straight paralleldislocations of density ., it has the approximate correlation properties

h%"i ! 0, %"#r, !$%" r" r0, ! " ! 0+ ,% &! %"2

% &f" r0='", !

0=!c+ ,

, #42$

where h%"2i - G2b2., '" - 1=---.

pis the correlation length of the fluctuating stress

field created by the dislocations, and f" is a non-dimensional correlation functionwith characteristic ranges '" and !c in its respective arguments. The ‘correlationstrain’ !c - b

---.

pwas estimated as the strain accomplished when all dislocations

move by the average dislocation spacing (for details see [76, 78] and referencestherein). Hardening may be introduced into the model by allowing the dislocationdensity and, hence, the amplitude h%"2i of local stress fluctuations to increase withlocal strain. In particular, linear hardening corresponds to a quadratic increase ofdislocation density with stress and strain. The term C!xx in equation (41), in whichC - G=., stems from the short-range interactions between discrete dislocationsmoving on close slip planes (for derivation of this term, see Groma et al. [79]).This second-order gradient term scales in Fourier space like k2!#k$ and is,hence, on large scales irrelevant in comparison with the long range elastic term,equation (39). However, the second-order gradient term has a decisive influenceon the small-scale morphology of the deformation patterns, as it breaks the symme-try existing in the kernel in equation (38) between the x and y directions, andsuppresses deformation heterogeneities in the direction of dislocation glide.

226 M. Zaiser

Downloaded By: [Karlsruher Inst fur Technologie Kit] At: 14:00 9 December 2010

This turns out to be crucial for describing striated deformation patterns similar tothe slip-line patterns observed in experiment.

The dynamics of the constitutive model specified by equations (38)–(42) exhibitsa transition between a pinned and a moving phase, which corresponds to thedepinning of an elastic manifold described by the equation

$@t! ! " " "int " C!xx " %"#!, r$: #43$

To see the analogy, we assume without loss of generality that the applied stress "in equations (40) and (43) is positive and note that, apart from initial transientsdue to initial conditions, the local strain in both models increases monotonicallyunder a positive stress. Hence, under a constant or increasing applied stressboth equations yield the same asymptotic dynamics. In the hypothetical case ofcolumnar disorder where the fluctuating stress %" is a function of x and ! only, !becomes independent on y, the internal stress "int vanishes, and elasticity iscontrolled by the second-order gradient term. In this case, the model becomesformally equivalent to the motion of a 1D manifold with local elasticity (a! 2) ina disordered medium. In the general case considered in the following, %" dependson both x and y, and the elastic behaviour is on large scales governed bythe long-range kernel of equation (38). Since a! 0 for this kernel, irrespectiveof space dimensionality one expects mean-field behaviour of the depinningtransition.

We note that, even though part of the above discussion is specific to fluctuatinginternal stresses generated by crystal lattice dislocations, the general form of ourequations is generic and can be applied to any material: The term %"#r, !$ – which ingeneral may have non-zero average – statistically represents microstresses on thescale of the discrete elements whose dynamics governs plastic deformation, andthe coupling term C!xx (more generally )rCr+!) approximately describes short-range interactions on the scale of the size or spacing of these discrete elements.It is therefore not astonishing that the present constitutive formulation has manysimilarities with models of the plastic flow of amorphous solids and ‘yield-stressliquids’ as proposed by Barat et al. [80], Bulatov and Argon [81], and Picard et al.[82]. The model of Barat et al. generalizes ideally plastic behaviour to a material withrandom microstructure and microstructure evolution; the main di"erence with thepresent model – apart from the assumption of an extremal dynamics instead of linearviscoplasticity – is a di"erent deformation geometry (plane vs. antiplane shear). Themodels of Bulatov and Argon, and Picard et al. on the other hand, use slightlydi"erent constitutive models for which yielding is associated with a strain softeninginstability.

3.2.2. Avalanche dynamics and surface morphology evolution.Stress–strain curves and slip avalanches Stress–strain curves obtained from simula-tions of the continuum model detailed in the previous section are shown in figure 19.In this and in the following figures, length, stress, and strain are again measured inthe respective ‘natural units’ 1=

---.

p, Gb

---.

p, and b

---.

pfor a dislocation system. In the

case of simulations with hardening, the hardening coe!cient d"=d! is accordinglymeasured in units of G, and the dislocation density . entering these scaling factorsis understood as the initial density. All simulations are carried out with periodic

Scale invariance in plastic flow of crystalline solids 227

Downloaded By: [Karlsruher Inst fur Technologie Kit] At: 14:00 9 December 2010

boundary conditions. It is seen from figure 19 that the simulated stress–strain graphsexhibit the same staircase-like characteristics as those observed in 2D dislocationdynamics simulations (figure 16). In the absence of hardening, the strain diverges atsome critical stress "c where the stress–strain curve reaches a horizontal tangent.Averaging over many stress–strain curves shows that the susceptibility - ! @!=@"of the plastic strain diverges according to - / #"c % "$%1, in the same manner asfor the discrete dislocation model discussed in section 3.1.4 and in line with theexpectation for mean-field depinning.

Close to the critical stress, the stress–strain curves have the structure of a ‘devil’sstaircase’ where the step sizes (sizes of slip avalanches) obey a scale-free distribution.Figure 20 shows distributions of step sizes $! obtained over narrow stress intervals(width 0.01 in scaled variables) and at various distances from the critical stress. Asone approaches the critical stress, the power-law scaling p#$!$ / $!%, with , - 1:4extends over a larger and larger range of scales, with the maximum size of the slipavalanches diverging like #"c % "$%2.

This behaviour is almost identical with that observed in the 2D dislocationdynamics simulations reported in section 3.1.4 (figure 18) and again the avalancheexponent , may be favourably compared with the exponents deduced from deforma-tion of micron-scale samples and from AE measurements. In fact, not only the shapeof the distributions but also the absolute avalanche sizes are practically the sameif one uses the relation $! ! bLtot=L

2s with Ls ! 256.%1=2 to convert between data in

figures 20 and 18. This makes it plausible that both models, though conceptuallydi"erent in their formulation, not only belong to the same universality class butdescribe the same physical reality.

Figure 21 shows avalanche size distributions determined for di"erenthardening rates and stresses above the critical stress (macroscopic yield stress) of

0 5 10 15 20 25 30 35 400.10

0.15

0.20

0.25

0.30

stre

ss [G

b,01/

2 ]

plastic strain [b,01/2]

2.5 3.0 3.5 4.0 5.00.24

0.25

0.26

stre

ss[G

b,01/

2 ]

strain[b,01/2]

Figure 19. Stress–strain curves as obtained from simulation of a system of size 128* 128with zero hardening (lower curve) and with non-dimensional hardening coe!cient of3:5* 10%3 (upper curve); insert: detail of the same stress–strain curves.

228 M. Zaiser

Downloaded By: [Karlsruher Inst fur Technologie Kit] At: 14:00 9 December 2010

a non-hardening system. It is obvious from figures 19 and 21 that hardening does not

fundamentally change the stepwise morphology of the stress–strain curves or the

power-law statistics, but eliminates the largest avalanches which, in a non-hardening

system, occur at stresses close to the critical stress. In this sense, hardening

suppresses the critical behaviour associated with the critical stress "c, but neverthe-

less leaves many of the scale-invariant properties of the dynamics unchanged.

10$7 10$6 10$5 10$4 10$3 10$210$7

10$6

10$5

10$4

10$3

10$2

10$1

100

101

102

1-!ext/!C=0.11-!ext/!C=0.21-!ext/!C=0.31-!ext/!C=0.4pr

obab

ility

den

sity

p('

")/(

1-! e

xt/!

c)2

scaled strain increment (1-!ext/!C)2'"10$5 10$4 10$3 10$2 10$1 100

10$9

10$8

10$7

10$6

10$5

10$4

10$3

10$2

10$1

100

prob

abili

ty d

ensi

ty p

('") &=1.4

1-!ext/!C=0.11-!ext/!C=0.21-!ext/!C=0.31-!ext/!C=0.4

strain increment '" [b,1/2]

Figure 20. Probability distributions of slip avalanche sizes (probability density p#$!$ vs.strain increment $!) as obtained from an ensemble of systems of size 256*256; left: distribu-tions corresponding to di"erent stresses; right: universal distribution obtained by re-scaling$! ! $!#1% "="c$2.

10$7 10$6 10$5 10$4 10$3 10$2 10$1 10010$9

10$8

10$7

10$6

10$5

10$4

10$3

10$2

10$1

100

# = 0.002# = 0.004# = 0.008# = 0.016# = 0.032

prob

abili

ty d

ensi

ty p

('")

strain increment '" [b,1/2]

10$9 10$8 10$7 10$6 10$5 10$4 10$3

10$7

10$6

10$5

10$4

10$3

10$2

10$1

100

101

102

# = 0.002# = 0.004# = 0.008# = 0.016# = 0.032

prob

abili

ty d

ensi

ty p

(#'"

)

Scaled strain increment #'"

Figure 21. Probability distributions of slip avalanche sizes; left: distributions correspondingto di"erent hardening rates; right: universal distribution obtained by re-scaling $! ! #$!.

Scale invariance in plastic flow of crystalline solids 229

Downloaded By: [Karlsruher Inst fur Technologie Kit] At: 14:00 9 December 2010

The fact that the avalanche exponent , - 1:4 is not changed by hardening compareswell with the observations of Richeton et al. [45] on single crystals of hcp metals:During hardening stages I and II, the energy exponent ,E - 1:5 was found to remainunchanged in spite of strongly di"ering hardening coe!cients.

According to figure 21, in a strain-hardening system, the size of the largest slipavalanches is inversely proportional to the hardening coe!cient. This can be easilyunderstood from a scaling argument. With an avalanche exponent of , - 1:5, theaverage strain $! in an avalanche follows the relation h$!i / $!1=2

max. Due to hard-ening, each avalanche raises the critical stress by a small amount $"c / #h$!i, whichimplies that the external stress (which cannot instantaneously follow) lags behindthe current critical stress by a similar amount. Finally, the maximum avalanche sizefollows the scaling relationship $!max / #"c % "$%2. Combining these relations, itfollows directly that $!max / 1=#. We note that a very similar observation wasmade by Zapperi et al. regarding the influence of a demagnetizing factor on themotion of domain walls driven by an applied magnetic field through a disorderedferromagnet [26].

The hardening coe!cients used in figure 21 (#=G ! 0:002, . . . , 0:032) tend to beabove the range of hardening coe!cients observed in single-slip deformation experi-ments on metal single crystals (#=G ! 10%4, . . . , 5* 10%3); the reason for this issimply that for smaller hardening coe!cients the cut-o" of the simulated avalanchesize distributions becomes independent of #, since it is then limited by the system sizeand not by the intrinsic dynamics of the system.

The stress–strain curves and avalanche statistics obtained from the time-continuous equation (40) are very similar to those obtained in [76, 78] from anautomaton version of the same model, where the strain on the sites of a grid ofunit mesh length was increased by a unit amount, and a new randomly chosen yieldstress was assigned to that site, whenever the local stress exceeded the local yieldstress. (The only perceptible di"erence between both models is that in the automatonmodel the critical stress is ca 20% higher for the same yield stress distribution.)However, the time-continuous model gives access to additional information interms of the distribution of peak strain rates _!max !: A (evidently, a strain rate isdi!cult to define in an automaton model). Again, one observes a power lawp#A$ / A%,A with ,A - 2, in good agreement with the peak amplitude distributionof AE bursts in ice (section 2.1). Irrespective of the hardening rate, no cut-o" to thescale-free behaviour is apparent (figure 22).

Slip pattern and surface roughening Numerical simulation of the continuum modeldefined by equations (40)–(42) yields strongly anisotropic, striated strain patterns(figure 23) with strong correlations in the x direction (the direction of the slip plane)but weak correlations in the normal direction. This can be readily understood bylooking at the elastic interactions in Fourier space: The Fourier transform of theelastic kernel is zero along the kx and ky directions, see equation (39). While fluctua-tions along the kx direction are damped due to the second-order gradient term inequation (41), those along the y direction are not. The model is, hence, capable ofrepresenting at least qualitatively the slip anisotropy which in real crystals is a directconsequence of the glide motion of dislocations on slip planes.

230 M. Zaiser

Downloaded By: [Karlsruher Inst fur Technologie Kit] At: 14:00 9 December 2010

To compare with experimental findings (cf. section 2.2), one may integrate thestrain profile along the y direction for some fixed x ! x0 to obtain a displacementprofile along the corresponding plane normal to the slip direction:

y#x$ !"x

0)!#x$ % h!i+dx: #44$

1 10 100

1E-5

1E-4

1E-3

0.01

0.1

1

#=1.4x10$4

#=7.0x10$4

#=3.5x10$3

prob

abili

ty d

ensi

ty p

(A)

peak strain rate A [arbitrary units]

Figure 22. Probability distribution of peak strain amplitudes A ! _!max obtained for di"erenthardening rates. The distributions can be well approximated by a power law, p#A$ / A%2.

0 20 40 60 80 1000

20

40

60

80

100

X

Y

66.50 -- 70.0063.00 -- 66.5059.50 -- 63.0056.00 -- 59.5052.50 -- 56.0049.00 -- 52.5045.50 -- 49.0042.00 -- 45.5038.50 -- 42.0035.00 -- 38.5031.50 -- 35.0028.00 -- 31.5024.50 -- 28.0021.00 -- 24.5017.50 -- 21.0014.00 -- 17.5010.50 -- 14.007.000 -- 10.503.500 -- 7.0000 -- 3.500

Figure 23. Strain pattern obtained after simulation of a system of size 256* 256 to anaverage strain of 20b

---.

p(slip direction from left to right); greyscale: local strain in units

of b---.

p.

Scale invariance in plastic flow of crystalline solids 231

Downloaded By: [Karlsruher Inst fur Technologie Kit] At: 14:00 9 December 2010

Assuming that surface-specific e"ects can be neglected (near a free surface, the elasticinteractions are modified by the surface boundary conditions which are not takeninto account in our model), the morphology of such simulated ‘surfaces’ may becompared with that of real ones.

Analysis in terms of self-a!ne roughness was performed by studying the height–height correlation function and the power spectrum of the simulated surfaces [76].The results can be summarized as follows (see figure 24):

. The surfaces are self-a!ne up to a correlation length which is proportionalto the size of the simulated system. They can be characterized by a strain-independent roughness exponent * - 0:7.

. Increasing the total strain leads to growth of the profiles but does not changethe roughness exponent or the correlation length (which is anyway determinedby the system size). At large strains, the rms surface roughness on a given scalegrows as the square root of strain.

. The numerical value of the roughness exponent compares well with the experi-mental observations, whereas the growth exponent of about 0.5 is slightlybelow the exponent of 0.8 observed during the single-slip deformationStage I of KCl single crystals.

As discussed in section 2.2, self-a!ne surface roughness with a non-trivialroughness exponent * > 0:5 points towards long-range correlations in the strainfluctuation pattern, with a strain fluctuation correlation function which decays liker2*%2. To elucidate the nature of such correlations in our simulations, it is useful

1 10 100 1000100

101

102

103

104

105

2H=1.4

Mea

n sq

uare

hei

ght d

iffer

ence

[b2 ]

Horizontal spacing

1E-3 0.01 0.11$3

$2

$1

0

1

2

3

$2H-1=2.5Log(

P(k

))

k [arbitrary units]

Figure 24. Mean square height di"erence vs. horizontal distance for surface profiles obtainedfrom a system of size 512* 512 after simulation to average strains of 6b

---.

pand 20b

---.

p; each

graph has been averaged over 10 simulated profiles; insert: Average power spectrum of thesimulated surfaces for ! ! 20b

---.

p.

232 M. Zaiser

Downloaded By: [Karlsruher Inst fur Technologie Kit] At: 14:00 9 December 2010

to investigate the spatial distribution of slip in an avalanche. A greyscale image ofthe slip distribution in a large avalanche is shown in figure 25. The slip distributionon small scales is characterized by striations parallel to the x axis. At the same time,long-range correlations are visibly evident both in the x and in the y directions.

These correlations can be quantified by calculating the correlation integralC#R$ !

*jr%r0 j<Rh$!#r$$!#r0$id2#r% r0$. A power-law increase C#R$ / RD of the

correlation integral with non-integer D points towards a fractal pattern. Fromfigure 26 one sees that linear scaling is approximately observed in large avalanches,with an apparent dimension of D ! 1:7. Since the overall strain pattern isgoverned by the largest avalanches, this corresponds to a decay of the strain–straincorrelation function like r%0:3 which is consistent with a roughness exponentaround 0.7.

3.3. Phase-field models

Phase-field models have an intermediate position between dislocation-based andcontinuum approaches towards plastic flow modelling. Similar to continuumapproaches, the plastic deformation state is described by the evolution of strainvariables. However, the strains are resolved on a ‘microscopic’ scale on whichindividual dislocations appear as localized gradients in the shear strain fields onthe respective slip systems. The evolution of the local shear strains is derived froman elastic energy functional which includes not only long-range elasticity but also thePeierls energy of the crystal. The Peierls energy reflects the periodic structure of theatomic lattice and ensures that, in a stress-free crystal, the local shear strains take

16 32 48 64 80 96 112 128

16

32

48

64

80

96

112

128

X

Y

0.1

0.2

0.4

0.8

1.6

3.2

6.4

12.8

12.8

Figure 25. Strain distribution in a typical avalanche in a system of size 128* 128 (greyscalevalues of local strain in units of b

---.

p; the total strain increment in this avalanche averaged

over the entire system is $! ! 0:5b---.

p.

Scale invariance in plastic flow of crystalline solids 233

Downloaded By: [Karlsruher Inst fur Technologie Kit] At: 14:00 9 December 2010

discrete values corresponding to displacements by multiples of the Burgers vectorsof the respective slip systems.

Due to the description of the lattice strain on a quasi-atomic scale, the distinctionbetween the stress (or the elastic strain) and the plastic strain becomes meaningless:Both quantities are described by the same variable, namely the relative displacementbetween two slipping lattice planes divided by their separation. We discuss in somedetail the model proposed by Koslowski et al. [83, 84], who consider deformation ona single slip system and have applied their model to avalanche phenomena. Thismodel envisages the two-dimensional distribution of slip on a single slip plane z! 0in a three-dimensional continuum. (It is important to note that phase-field modelsare not restricted to single slip or planar systems. Phase-field modelling of multipleslip in three spatial dimensions, and the relation with 3D dislocation dynamics, hasbeen discussed by Katchaturyan and co-workers [85]. The numerical simulation ofsuch models is at present, however, computationally even more expensive than 3Ddislocation dynamics simulations.)

Starting out from a continuous elastic–plastic shear strain field and a piecewiseparabolic Peierls potential, Koslowski et al. [84] derive a formulation in which theplastic deformation field !#x, y$ is represented as an integer-valued field with time-discrete dynamics. The deformation field at time i" 1 is obtained from the fieldat time i by minimizing the incremental work function

W )!#x, y, i" 1$j!#x, y, i$+ ! E )!#x, y, i" 1$+ % E )!#x, y, i$+

""f#x, y$j!#x, y, i" 1$ % !#x, y, i$jdxdy #45$

100 101 102100

101

102

103

104

100<'"Ls2<200

1000<'"Ls2<2000

10000<'"Ls2<20000

Cor

rela

tion

inte

gral

radius r

Figure 26. Correlation integrals of the strain distribution in avalanches of di"erent size; thestraight line has slope D! 1.7.

234 M. Zaiser

Downloaded By: [Karlsruher Inst fur Technologie Kit] At: 14:00 9 December 2010

where E )!#x, y, i" 1$+ is the elastic energy functional which in the presence ofan external stress field "#r$ is given by

E )!+ ! Gb2

4

"K

1" Kdp=2j!#k$j2 " "#k$b!#k$

1" Kdp=2

! .d2k

#2p$2: #46$

Here, "#k$ and !#k$ are Fourier transforms of the fields "#r$ and !#r$, dp is theinterplanar spacing, and

K !k2y---------------

k2x " k2y

q " 1

1% +

k2x---------------k2x " k2y

q : #47$

The term f(x, y) in equation (45) denotes the energy that is dissipated in changing thestrain at the point (x, y) by a unit amount; it plays the role of a local obstacle strengthwhich in [84] was assumed as a sum over randomly distributed point obstacles.

A detailed derivation of this model, starting from a continuous strain field and anenergy functional with a piecewise parabolic Peierls potential, is given in [83]. Herewe exclusively discuss the avalanche dynamics exhibited by the model as addressedin [84]. As an initial condition, Koslowski and co-workers in that paper assume astrain- and dislocation-free crystal under zero external stress. By increasing theexternal stress by small amounts and carrying out a sequence of minimizationsteps of the work functional given by equation (45), they demonstrate that theensuing time-discrete dynamics exhibits a series of strain bursts with scale-invariantsize distribution, with an approximately stress-independent exponent ,! - 1:8 forthe distribution of strain increments.

While this is in itself an interesting finding and compares reasonably well withexperimental observations, one objection may be raised against the procedureapplied in these calculations. The discrete dynamics defined by equation (45) samplesa sequence of energy minima but does not tell how the system gets from one mini-mum to another. That this may be a problem can be seen immediately by envisagingthe moment when, under an increasing applied stress, the very first dislocationappears in the system. This happens as soon as the energy of a dislocation loop,trapped at obstacles somewhere in the system, falls below that of the dislocation-freecrystal – a situation bound to be happen sooner or later since the loop, once created,reduces the elastic energy of the system by an amount proportional to the appliedstress times the loop area. However, since the initial configuration is a dislocation-free crystal and only one slip plane is considered, dislocation sources do not exist andthe loop has to be created ex nihil. It is easy to demonstrate that this process requiresto overcome an energy barrier of prohibitive height, unless the applied stress is closeto the theoretical shear strength of the ideal crystal. The model of Koslowski et al.does not ‘see’ this problem since it samples energy minima irrespective of theexistence or non-existence of a path connecting them.

In spite of this flaw, the model has several interesting features. Spatial andtemporal coarse-graining of the discrete-time dynamics given by equations(45)–(47) leads to

@!#x, y$@t

! %E 0#!$%!

" f#x, y, !$ #48$

Scale invariance in plastic flow of crystalline solids 235

Downloaded By: [Karlsruher Inst fur Technologie Kit] At: 14:00 9 December 2010

where the coarse-grained energy functional E 0 is given by

E )!#x, y$+ ! Gb2

4

"Kj!#k$j2 " "#k$b!#k$/ 0 d2k

#2p$2: #49$

Equation (48) is the equation of motion of a two-dimensional manifold with long-range elasticity (the interaction kernel scales in proportion with the wavevectormodulus k) moving through a random medium as characterized by the randomdissipative force f. As discussed in the introduction, this model (a ! 1, d ! 2) isin the universality class of mean-field depinning. In fact, the motion of a two-dimensional pile-up of flexible dislocations as studied by Moretti et al. [27], whichwas found to be in the same universality class, can be treated within the frameworkof Koslowski et al. by using as initial condition for the strain field a constant straingradient. The avalanche exponent observed by Koslowski and co-workers is some-what above the value , ! 1:5 expected for mean-field depinning. The reason for thisdi"erence is not completely clear – it may be that Koslowski et al. include in theirstatistics events from the microplastic region well below the yield stress, whichleads to an apparent increase of the avalanche exponent (cf. the discussion afterequation (36)). It could also be that the di"erence is simply due to a technicality,since in [84] a linear instead of logarithmic binning procedure is used.

The model of Koslowski et al. provides a conceptual bridge between dislocation-based and strain-based models. As it stands, the model needs to introduce quencheddisorder (the random dissipative force f(x, y)) in order to obtain metastabledislocation configurations. It remains a task for future work to generalize themodel to more than one slip plane and investigate the possibility of self-pinning ofthe dislocation system in the absence of quenched disorder, which characterizes thediscrete dislocation dynamics simulations discussed in section 3.1.

4. Discussion and conclusions

From the experimental and theoretical considerations discussed in the presentreview, a picture of crystal plasticity emerges which is at variance with the traditionalparadigm of plasticity as a laminar flow process. The key elements of this picturemay be summarized as follows:

(1) Plastically deforming crystals can under usual experimental conditions beenvisaged as slowly driven non-equilibrium systems. The notion of ‘slow’requires, however, some specification. This will be discussed in detail below.

(2) The dynamics of these systems is governed by the presence of a critical pointmarking a non-equilibrium phase transition (‘yielding transition’) of thedislocation system where, at a critical applied stress, the dislocations passfrom a pinned/jammed to a moving phase.

(3) Critical behaviour manifests itself in terms of strongly intermittent dynamicswith bursts of activity (‘deformation avalanches’) separated by quiescentintervals. The sizes of the avalanches obey scale-free distributions, character-istic of the intermittent ‘crackling noise’ associated also with other dynamicalcritical phenomena [46]. Both the spatial and the temporal distribution of the

236 M. Zaiser

Downloaded By: [Karlsruher Inst fur Technologie Kit] At: 14:00 9 December 2010

avalanches are characterized by long-range correlations (spatial clustering,emergence of ‘aftershocks’). There are indications that the spatial distribu-tion of slip events follows fractal patterns [7, 48]. Scaling properties can alsobe observed in surface patterns where a self-a!ne surface morphologyemerges during deformation.

(4) Observations of scale-free behaviour can be made on a wide class of metalsand alloys. Details of crystal structure and alloy composition seem to belargely irrelevant – for instance, in the present review we find that thesame model (section 3.2) can explain experimental observations made onice, alkali halides, pure fcc metals, and superalloys. This robustness mayindicate universality associated with the behaviour near the ‘yieldingtransition’. Many of the theoretical and experimental results compiled inthe present review indicate that this critical behaviour could simply be inthe universality class of mean-field depinning.

It is obvious that this picture of plasticity owes a lot to the recent availability ofconvincing experimental data, in particular to the very comprehensive investigationsof AE activity in ice carried out by Weiss and co-workers [6, 7, 36–41]. Given the factthat this as well as most of other experimental work reported in the present reviewuses techniques that have been available for decades, one may ask why the intriguingcollective behaviour that can be observed during plastic deformation of crystals hasescaped the attention of the physics and materials science communities until veryrecently.

4.1. Why has it not been seen before?

Some general observations A first and obvious response to this question leads usinto the field of sociology (and psychology) of science. People tend to look forphenomena which they expect and understand, in other words, phenomena forwhich there is a conceptual and interpretative framework. A good scientist reportswhat he sees, but in the absence of such a framework, it is only too likely that someobservations may not be followed up. In fact, jumps of the local strain which closelymatch the ‘staircase-shaped’ stress–strain curves of micron-scale samples (see section3.1.3 and references) have been reported in the 1970s [60] and possibly even earlier.The experiments discussed in section 2.2.1, which demonstrated fractal slip patterns,date from the mid-1980s [48]. But only since the late 1980s has a conceptual frame-work been developed in which avalanche dynamics, crackling noise, and scale-freestatistics are perceived as fairly general phenomena which are characteristic of awide class of driven non-equilibrium systems. In the absence of such a framework,occasional observations of large fluctuations and scale-free behaviour reported in thematerials literature remained unexplained and to some extent inconsequential.

In case of acoustic emission measurements, the situation is further complicatedby the space and time scales involved. In the following it will be demonstrated that,depending on strain rate, hardening rate and dislocation density such measurementsmay yield either discrete or continuous AE signals, or a superposition of both, inspite of the fact that the underlying dynamics on microscopic and mesoscopic scalesis the same in either case. Given the lack of explanation of ‘crackling’ signals, it istherefore quite natural that early research has usually focused on the continuous AE

Scale invariance in plastic flow of crystalline solids 237

Downloaded By: [Karlsruher Inst fur Technologie Kit] At: 14:00 9 December 2010

as discussed in section 2.1.3. Even in cases where the crackling nature of the signalcannot be overlooked, as in the example shown in figure 5, no statistical analysis wasperformed since scale-free noise statistics were not considered a relevant or topicalissue. In the opinion of the present author, however, continuous and discontinuousAE signals recorded during deformation of metals and alloys relate to the samefundamental physical processes which in ice single- and polycrystals give rise to anintermittent ‘crackling’ noise. We will show in the following why in metalsdiscontinuous AE is often masked by an overlapping of signals emanating fromdi"erent deformation bursts which is caused by the e"ect of a finite driving rate.

Deformation rate e"ects and the transition from discrete to continuous AE signals Inplastic deformation of metals, one often observes transitions between discrete andcontinuous acoustic emission signals, as well as the simultaneous occurrence of both(spikes above a continuous background), cf. section 2.1.3 and figure 5. In this case,the continuous part of the signal may simply stem from the superposition of acousticwaves originating from independent bursts at di"erent locations in the specimen.To assess the conditions under which this may occur, we consider a strain-ratecontrolled deformation test and define two critical strain rates: Above a criticalstrain rate _!1, the average time between two events falls below the mean eventduration and a continuous background appears. At a second critical strain rate_!2, the magnitude of the continuous background becomes of the same order ofmagnitude as the characteristic amplitude $!max of the largest bursts. Above thisrate, crackling noise becomes altogether unobservable. If we make the simplifyingassumptions that bursts occur uncorrelated in time, and the amplitudes of subse-quent burst are statistically independent, these two critical strain rates can be esti-mated as

_!1 !h$!itr

, _!2 !$!max

h$!i_!1 !

h$!maxitr

: #50$

Here tr denotes the e"ective duration of a burst as recorded by the acoustic trans-ducer. Because of reflections at the specimen surfaces, this duration is in generallonger than the actual duration of the burst. A lower estimate for tr is therefore givenby the characteristic time for acoustic wave propagation, tr 2 c=Ls where Ls is thecharacteristic size of the specimen and c the longitudinal sound wave velocity. Wefinally note that, for stress controlled experiments, critical stress rates can be definedas _"1=2 ! # _!1=2 where # is the strain hardening coe!cient or the inverse susceptibility,# ! #@h!i=@"$%1.

For a power-law burst size distribution with exponent 1 < , < 2 and upperand lower cut-o" $!max and $!min, the average strain increment in a burst is

h$!i ! 2% ,

,% 1$!2%,

max$!,%1min : #51$

It is easy to see that, for a truly scale-free distribution where the upper cut-o"diverges, the burstlike signal can always be observed. On the other hand, ourinvestigation in section 3 has demonstrated that the distribution of event sizes isusually truncated at some large cut-o" size. Such a cut-o" in reality always exists.It may be due to intrinsic reasons (the stress is below the yield stress, or the material

238 M. Zaiser

Downloaded By: [Karlsruher Inst fur Technologie Kit] At: 14:00 9 December 2010

exhibits strain hardening, cf. section 3.2). It may also result from the e"ects of finitegrain size, or simply from the finite size of the deforming specimen.

Here we focus on the situation which is most relevant for assessing the observa-bility of intermittent AE bursts in conventional deformation experiments, namely asingle crystal of macroscopic dimensions which is deformed in strain rate control.(In polycrystals, the maximum event sizes are expected to be smaller and thereforebursts may be more di!cult to observe.) We consider the upper critical strain rate _!2which according to equation (50) depends on the maximum event size only. At lowerstrain rates, superposition of events may a"ect the statistical characteristicsof the AE signal even though the ‘crackling’ nature of the signal is still manifest.For a discussion of these e"ects the reader is referred to the work by White andDahmen [86].

We consider large events as a cascade of elementary ones, $!max ! Nmax$!min.If plastic flow is controlled by dislocation interactions, the volume occupied by thesmallest events is expected to be of the order of .%3=2 and the strain produced withinthis volume to be of the order of b.1=2 where . is the dislocation density (onedislocation segment moves by one ‘wavelength’ of the internal stress field, cf. thescaling relations discussed in section 3.1.1). The strain produced by an ‘elementaryevent’ within the macroscopic volume Vs of the deforming body is then given by$!min ! b=.Vs. The number Nmax does not depend on the dislocation density . butis, as discussed in section 3.2, inversely proportional to the strain hardeningcoe!cient: Nmax ! CG=#. From the simulation results of section 3.2 we obtain theestimate C - 50.

Throwing together all these relations, we can estimate the critical strain ratebelow which intermittent ‘crackling’ noise can be observed. We find that

_!2 -CbcG

#VsLs.: #52$

We consider a Cu specimen with typical dimensions Ls - V1=3s - 5 mm, Burgers

vector length of b ! 2:5 A, and typical dislocation densities and hardening coe!-cients in hardening stages I and II. In Stage I, #=G - 5* 10%4 and . - 1012 m%2

which yields a value _!2 - 2:5* 10%4 s%1 which is well within the usual range usedin deformation tests. In Stage II, on the other hand, typical dislocation densities areone or two orders of magnitude larger and the hardening coe!cient increases by upto a factor of 10, #=G - 5* 10%3 and . - 5* 1013 which leads to a critical strainrate _!2 - 5* 10%7 which is well below the usual experimental range. These estimatescompare well with observations of Imanaka et al. [42] who observed burstlike AEduring the initial loading of a Cu single crystal of high purity and very low initialyield stress (" < 1MPa) which after deformation to a flow stress of about 3MPa(corresponding to a tenfold increase in dislocation density) gave way to a continuousAE signal. The observation of crackling noise in hcp metals, where Stage IIdislocation densities and hardening rates tend to be lower than in fcc metals, fitsinto the same picture, as does the fact that Weiss et al. made their observations onice single crystals with extremely low initial dislocation densities (. / 108 m%2).

These estimates indicate that observability of burstlike AE induced by disloca-tion plasticity can under usual experimental conditions not be taken for granted evenin fcc metals where dislocation mobilities are high. The situation may be di"erent in

Scale invariance in plastic flow of crystalline solids 239

Downloaded By: [Karlsruher Inst fur Technologie Kit] At: 14:00 9 December 2010

deformation by twinning, where the elementary events are much larger, and/or inthe presence of plastic instabilities. However, our estimates also demonstrate thatmacroscopically continuous AE signals need not be at variance with an intermittentavalanche dynamics on mesoscopic and microscopic scales which, in the case of thesimulation data of figure 21 on which our estimate is based, exhibits scale-freebehaviour over five orders of magnitude in avalanche size.

4.2. Open questions, doubts and prospects

In this review we argue that scale-free fluctuation patterns in crystal plasticity repre-sent critical behaviour associated with a non-equilibrium critical point (‘yieldingtransition’). However, critical behaviour is by definition confined to an isolatedpoint in parameter space: critical phenomena are not generic. Furthermore, aplastically deforming crystal is not actually in a steady state: Since plasticity leadsto microstructural changes (dislocation multiplication, strain hardening), ongoingdeformation requires an continuously increasing stress. Hence, in strain hardeningmaterials (i.e. in most crystalline solids) the point of yielding, in the sense of sus-tained flow under constant stress, is actually never reached: If the yield stress marksa critical point, the system chases the ghost of that point as each stress incrementleads to plastic activity which in turn, due to the ensuing microstructural changes,moves the point of yielding towards higher and higher stresses.

There are two ways to reconcile these observations with the fact that, as demon-strated in this review, scale-free fluctuations are a fairly general feature of crystalplastic flow:

(i) Several authors have adopted the notion of self-organized criticality (SOC).SOC in the context of plasticity means that there is some mechanism which ensuresthat the evolving dislocation system settles into a state where the applied stresscorresponds precisely to the momentary yield stress. Indeed, the model discussedin section 3.2 of the present review is closely related to a model proposed by Bak andco-workers for describing the ‘self-organized critical’ dynamics of shearing processesat earthquake faults [87]: The SOC model of Bak et al. actually implements anautomaton version of the continuum model in section 3.2, with a particular choiceof the hardening coe!cient. This observation, however, rather than advocating theconcept of SOC for plasticity, indicates that the model of Bak et al. is actually notevolving towards a truly critical state (cf. the discussion of hardening in section 3.2).The fact that Bak et al. in [87] do not find any intrinsic limits to the scaling regimes oftheir avalanche size distributions has the simple reason that their system sizes are toosmall. As a consequence, they find scaling over two decades, whereas our results insection 3.2 even for large hardening coe!cients indicate robust scaling over fourdecades before the intrinsic cut-o" proportional to the hardening coe!cient becomesmanifest.

(ii) The concept we prefer is that of ‘robust scaling’: the dynamics of a systemmay exhibit scaling behaviour associated with a critical point even if the system is notvery close to that point in parameter space. Our investigations have revealed severalexamples of such robust scaling – see, e.g. the avalanche size distribution in figure 18,where scaling behaviour over almost four decades is observed at stresses that are just20% of the critical stress.

240 M. Zaiser

Downloaded By: [Karlsruher Inst fur Technologie Kit] At: 14:00 9 December 2010

If plastically deforming crystals are not in a truly critical state, this has theimportant implication that, in su!ciently large samples, fluctuations will finallyaverage out. In terms of the acoustic emission, we have demonstrated that smalluncorrelated AE events from di"erent parts of the crystal may superimpose toproduce the continuous AE background commonly observed in AE experimentson metals and alloys. Similarly, in macroscopic deformation experiments thesuperposition of many small and uncorrelated strain increments obliterates the stair-case-like structure of the stress–strain curves that is blatantly manifest from smallsamples. Another implication of a possible absence of true criticality is that spatialcorrelations in the plastic flow pattern may have a finite range, above which thetraditional homogenization methods of continuum mechanics can be successfullyapplied. In fact, it may be wise to make the modest claims of ‘nearly critical’ or‘robust critical’ behaviour, as opposed to SOC, in order to avoid the impression thatthe methods of continuum mechanics (including homogenization methods and theuse of conventional constitutive equations in crystal plasticity) as used during thelast 200 years were completely o" the mark.

When it comes to predicting plasticity on the micron scale, as for instance inmicroelectromechanical systems, however, these caveats do not hold and conven-tional constitutive equations, which imply deterministic materials behaviour, mayindeed be quite inadequate to account for plastic behaviour which on these scales isintrinsically controlled by fluctuation phenomena.

Several observations still remain vexatious:

(1) In the creep experiments on ice, changing the stress over a wide range leavesthe energy distribution of AE bursts virtually unchanged, and no indicationof a cut-o" can be found over more than 6 decades in energy. Moreover, thesame distribution seems to govern the AE burst energies in di"erent creepregimes during which the average creep rates di"er by orders of magnitude.No presently available model seems capable of reproducing or understandingthis extremely robust behaviour. The ‘SOC viewpoint’ would of course bethat, whatever the stress, the system is self-organizing towards its criticalpoint. However, a physically motivated model which provides a mechanismfor such self-organization in a dislocation system has yet to be formulated.

(2) The interpretation of AE experiments hitherto relies on extremely simplisticmodels assuming compact sources. The theoretical investigations, on theother hand, indicate that the acoustic source during a ‘slip avalanche’ mayhave a complicated structure: owing to the long range of elastic interactions,dislocations may move in a correlated manner in spite of being widelyseparated, and the e"ective source may be a fractal dust rather than a com-pact object. One may ask whether the simplistic assumptions underlying thecurrent interpretation of AE measurements a"ect the results, in particularthe avalanche exponents. To clarify this point, one might investigate how thepredictions of an AE source model based on one of the models described insection 3 would di"er from those based on a simple coherent or incoherentsuperposition of compact sources as assumed in the analysis of previousexperiments.

Scale invariance in plastic flow of crystalline solids 241

Downloaded By: [Karlsruher Inst fur Technologie Kit] At: 14:00 9 December 2010

(3) All presently available models are formulated for single crystals and simpledeformation geometries, where the plastic strain and strain rate cane"ectively be treated as scalar fields and the stress as a scalar driving force.The same holds for many of the available experiments, which have beenconducted on single crystals deforming in single-slip geometries. The behav-iour of more general models which necessarily have to take into accountthe tensorial nature of stress and strain may be substantially di"erent, asthe dimensionality of the order parameter of the ‘yielding transition’ (i.e. thestrain rate) is evidently an important issue for any kind of critical behaviour.There is experimental evidence for di"erences between single and multipleslip in the acoustic emission signals recorded during deformation of ice poly-crystals, which di"er substantially from those recorded during single crystaldeformation: Not only does the size distribution of acoustic emission eventsin polycrystals exhibit a grain size dependent cut-o", but also the avalancheexponents are quite di"erent from those for single crystals. There may bedi"erent reasons for these observations: (i) Grain boundaries may act asdislocation obstacles, and the blocking of slip at grain boundaries maycause strong kinematic hardening, as well as overstresses in adjacent grains.This is especially pronounced in ice where the activation of other than basalslip systems is di!cult. (ii) In polycrystals (with the possible exception of ice),multiple slip systems operate simultaneously in most grains. To assess therespective influences of grain boundaries and multiple slip, both specificexperiments (e.g. on single crystals deforming in symmetrical multiple slip)and corresponding theoretical models are needed.

(4) Many aspects of the avalanche statistics seem to be consistent with mean-field depinning, and the results obtained from simulations of discretedislocation as well as of continuum models (section 3) point into the samedirection. This is not unexpected owing to the long-range nature of the elasticinteractions. However, the applicability of the depinning framework, andindeed the very existence of a unique depinning threshold (yield stress), isin no way guaranteed since the lack of positive definiteness of the interactionkernels prevents the application of Middleton’s ‘no passing’ theorem forproving the existence of a unique threshold [88].

(5) An important question concerns the relations between the spatial andtemporal structure of plastic flow. It is obvious that mean-field argumentsby definition cannot tell us anything about the spatial structure of a process.The investigations discussed in section 3.2 indicate that the stronglyanisotropic structure of the elastic kernels, which follows from continuumelasticity, may be crucial for the properties of strain patterns. Severalquestions remain unanswered: How can the observed spatio-temporalclustering of slip avalanches be explained? Can the existing models reproducethe fractal distribution of avalanche loci in a macroscopic sample asproposed in [7]? Is there a theoretical explanation of the observed surfaceroughening beyond the coincidence of experimental and simulation results?

A further issue which creates complications is the fact that the presentmodels tend to over-simplify the properties and the evolution of the crystal defect

242 M. Zaiser

Downloaded By: [Karlsruher Inst fur Technologie Kit] At: 14:00 9 December 2010

microstructure during deformation. The applicability of the depinning frameworkhinges on the presence of a statistically homogenous field of quenched disorder withshort-range correlations. In the present context this translates into the assumption ofa disordered and evolving, but at the same time statistically stationary dislocationmicrostructure. This assumption is acceptable in the sense that on the typical strainscale of individual slip avalanches the microstructure does not change a lot, and onthe strain scale where it does change, the slip avalanches are truncated due to theensuing hardening as discussed in section 3.2. Complications arise, however, fromthe following observations: Not only the dislocation density and the amplitude of theinternal-stress fluctuations increase during deformation, but at the same time thecharacteristic ‘wavelength’ of the dislocation microstructure, and the correlationlength of the stress fluctuations, decrease in proportion with the dislocation spacing.In the model of section 3.2, only the amplitude growth has been considered while thespatial ‘shrinking’ of the pinning field has been neglected. Another complicationstems from the fact that, under certain deformation conditions, dislocations mayarrange into fractal patterns, with a fractal dimension that increases during deforma-tion [9, 10]. This implies that the pattern of local yield stresses may itself possesslong-range correlations, and these correlations may not be stationary.

Many of the observations and models discussed in this review are not confinedto crystal plasticity, but apply to any kind of shear flow. Hence, it is not unexpectedthat the models discussed in the present review bear close relations to models used inother contexts. A prominent example is the model of Bak and co-workers ofearthquake dynamics [87] which is analogous to the continuum plasticity model ofsection 3.2. Another example is the amorphous materials plasticity model by Rouxet al. [80] which considers a di"erent deformation geometry (anti-plane instead ofplane shear) but can be translated into crystal plasticity language in a straightforwardmanner: The model corresponds to the antiplane shear of a 2D crystal lattice with twosymmetrical slip systems, while the other characteristics are essentially the same as inthe model of section 3.2. It is hoped that future systematic investigations of these andrelated models will yield a unified picture of the irreversible deformation ofboth crystalline and amorphous solids, which allows to analyse and classify boththe universal and the materials and geometry-specific features of plasticity.

Acknowledgments

M.Z. gratefully acknowledges numerous and stimulating discussions withS. Zapperi, J. Weiss, M.-C. Miguel, M. Alava, and E.C. Aifantis, as well as thecollaboration of J. Schwerdtfeger, E. Nadgorny, P. Moretti, F. Madani, andA. Konstantinidis. Finally, the hospitality of CNR, Istituto di Sistemi Complessi,Rome, Italy, during the period in which this review was written is gratefullyacknowledged.

References

[1] L.P. Kubin, Y. Estrin and E.C. Aifantis, Scripta Metall. Mater. 29 1147 (1993).[2] M. Zaiser and P. Hahner, Phys. Stat. Sol. (b) 199 267 (1997).

Scale invariance in plastic flow of crystalline solids 243

Downloaded By: [Karlsruher Inst fur Technologie Kit] At: 14:00 9 December 2010

[3] L.P. Kubin, C. Fressengeas and G. Ananthakrishna, in Dislocations in Solids, Vol. 11,edited by F.R.N. Nabarro and M.S. Duesbery (Amsterdam, North-Holland, 2002),pp. 101–192.

[4] M. Zaiser, Mater. Sci. Engng. A 309–310 304 (2001).[5] M.-C. Miguel, A. Vespignani, S. Zapperi, et al., Mater. Sci. Engng. A 309–310 324 (2001).[6] M.-C. Miguel, A. Vespignani, S. Zapperi, et al., Nature 410 667 (2001).[7] J. Weiss and D. Marsan, Science 299 89 (2003).[8] M. Zaiser, F. Madani, V. Koutsos and E.C. Aifantis, Phys. Rev. Lett. 93 195507 (2004).[9] P. Hahner, K. Bay and M. Zaiser, Phys. Rev. Lett. 81 2470 (1998).[10] M. Zaiser, K. Bay and P. Hahner, Acta Mater. 49 2463 (1999).[11] E.C. Aifantis, Int. J. Engng. Sci. 30 1279 (1992).[12] E.C. Aifantis, J. Eng. Mater. Tech. 121 189 (1999).[13] M. Zaiser and P. Hahner, Mater. Sci. Engng. A 238 399 (1997).[14] M. Zaiser and A. Seeger, in Dislocations in Solids, Vol. 11, edited by F.R.N. Nabarro and

M.S. Duesbery (Amsterdam, North-Holland, 2002), pp. 1–100.[15] J. Friedel, Dislocations (Pergamon Press, Oxford, 1967).[16] B. Devincre and M. Condat, Acta Metall. Mater. 40 2629 (1992).[17] S. Zapperi and M. Zaiser, Mater. Sci. Engng. A 309–310 348 (2001).[18] H. Leschhorn, T. Nattermann, S. Stepanow and L.H. Tang, Ann. Physik 6 1 (1997).[19] D.S. Fisher, Phys. Rep. 301 113 (1998).[20] P. Chauve, T. Giamarchi and P. Le Doussal, Phys. Rev. B 62 6241 (2000).[21] P. Le Doussal, K.J. Wiese and P. Chauve, Phys. Rev. B 66 174201 (2002).[22] R. Labusch, Cryst. Lattice Defects 1 1 (1969).[23] R. Labusch, Acta Metall. 20 917 (1972).[24] A.I. Lar’kin, and Yu.N. Ovchinnikov, J. Low Temp. Phys. 34 409 (1979).[25] F. Family and T. Vicsek, J. Phys. A, 18, L75 (1985).[26] S. Zapperi, P. Cizeau, G. Durin and H.E. Stanley, Phys. Rev. B 58 6353 (1998).[27] P. Moretti, M.-C. Miguel, M. Zaiser and S. Zapperi, Phys. Rev. B 69 214103 (2004).[28] D. Cule and T. Hwa, Phys. Rev. B 57 8235 (1998).[29] S. Ramanathan and D.S. Fisher, Phys. Rev. B 58 6026 (1998).[30] U. Nowak and K.D. Usadel, Europhys. Lett. 44 634 (1998).[31] L. Roters, A. Hucht, S. Lubeck, U. Nowak and K.D. Usadel, Phys. Rev. E 60 5202

(1999).[32] M. Paczuski, S. Maslov and P. Bak, Phys. Rev. B 56 414 (1996).[33] D. Rouby, P. Fleischmann and C. Duvergier, Phil. Mag. A 47 671 (1983).[34] D. Rouby, P. Fleischmann and C. Duvergier, Phil. Mag. A 47 689 (1983).[35] V.D. Natsik and K.A. Chishko, Sov. Phys. Solid State 20 1117 (1977).[36] J. Weiss and J.-R. Grasso, Phys. Chem. B 101 6113 (1997).[37] J. Weiss, F. Lahaie and J.-R. Grasso, J. Geophys. Res. 105 433 (2000).[38] J. Weiss, J.-R. Grasso, M.-C. Miguel, et al., 2001, Mater. Sci. Engng. A, 309-310, 360.[39] J. Weiss and M.-C. Miguel, Mater. Sci. Engng. A 387–389 292 (2004).[40] T. Richeton, J. Weiss and F. Louchet, Acta Mater. 53 4463 (2005).[41] T. Richeton, J. Weiss and F. Louchet, Nature Mater. 4 465 (2005).[42] T. Imanaka, K. Sano and M. Shimizu, Crystal Lattice Defects 4 57 (1973).[43] N. Kiesewetter and P. Schiller, Phys. Stat. Sol. (a) 38 569 (1976).[44] W. Scharwaechter and H. Ebener, Acta Metall. Mater. 38 195 (1990).[45] T. Richeton, P. Dobron, F. Chmelik, J. Weiss and F. Louchet, Mater. Sci. Engng. A,

submitted (cond-mat/0512301).[46] J.P.K. Sethna, A. Dahmen and C.R. Myers, Nature 410 242 (2001).[47] B. Sprusil and F. Hnilica, Czech. J. Phys. B 35 897 (1985).[48] T. Kleiser and M. Bocek, Z. Metallkde. 77 582 (1986).[49] H. Neuhauser, in Dislocations in Solids, edited by F.R.N. Nabarro (Amsterdam,

North-Holland, 1983), p. 319.[50] H. Neuhauser, Phys. Scr. T49, 412 (1993).[51] I. Simonsen, A. Hansen and O.M. Nes, Phys. Rev. E 58 2779 (1998).

244 M. Zaiser

Downloaded By: [Karlsruher Inst fur Technologie Kit] At: 14:00 9 December 2010

[52] E. Nadgorny, J. Schwerdtfeger, F. Madani, E.C. Aifantis and M. Zaiser, to appear inProceedings of the International Conference on Statistical Mechanics of Plasticity andRelated Instabilities, PoS (SMPRI2005)012.

[53] J.M. Lopez, M.A. Rodriguez and R. Cuerno, Phys. Rev. E 56 3993 (1997).[54] J.M. Lopez and J. Schmittbuhl, Phys. Rev. E 57 6405 (1998).[55] O. Wouters, J.P. Vellinga, J. Van Tijum, et al., Acta Mater. 53 4065 (2005).[56] M.D. Uchic, Mater. Sci. Engng. A 400–401 268 (2005).[57] M.D. Uchic, D.M. Dimiduk, J.N. Florando, et al., Science 305 986 (2004).[58] D.M. Dimiduk, M.D. Uchic and T.A. Parthasarathy, Acta Mater. 53 4065 (2005).[59] D.M. Dimiduk, C. Woodward, R. LeSar and M.D. Uchic, Science, submitted.[60] R.B. Pond, in The Inhomogeneity of Plastic Deformation (Metals Park, American Society

of Metals, 1973), p. 1.[61] A. Needleman and J. Gil Sevillano, Scripta Mater. 48 109 (2003).[62] E. Nadgorny, Dislocation Dynamics and Mechanical Properties of Crystals (Pergamon

Press, Oxford, 1988).[63] U. Essmann and H. Mughrabi, Phil. Mag. A 40 731 (1979).[64] M. Wilkens, Acta Metall. 17 1155 (1969).[65] F.F. Csikor, B. Kocsis, Bako, B. and I. Groma, Mater. Sci. Engng. A 400 214 (2005).[66] V.V. Bulatov, M. Tang and H.S. Zbib, 2001, Crystal Plasticity from Dislocation

Dynamics, MRS Bulletin, 26.[67] L. Kubin, Computer Modeling of Dislocation-Controlled Deformation, Encyclopedia of

Materials: Science and Technology (Amsterdam, Elsevier Science, 2001).[68] J. Gil Sevillano, E. Bouchaud and L.P. Kubin, Scripta Metall. Mater. 25 355 (1991).[69] M.-C.Miguel, A. Vespignani, M. Zaiser and S. Zapperi, Phys. Rev. Lett. 89 165501

(2002).[70] M.-C. Miguel, P. Moretti, M. Zaiser and S. Zapperi, Mater. Sci. Engng. A 400 191 (2005).[71] E.N. Andrade da C., Proc. R. Soc. London A 84 1 (1910).[72] E.N. Andrade da C., Proc. R. Soc. London A 90 329 (1914).[73] A. Pertsinidis and X.S. Ling, New J. Phys. 7 33 (2005).[74] M. Zaiser, B. Marmo and P. Moretti, in Proceedings of the International Conference on

Statistical Mechanics of Plasticity and Related Instabilities, PoS (SMPRI2005)053.[75] O. Perkovic, K. Dahmen and J.P. Sethna, Phys. Rev. Lett. 75 4528 (1995).[76] M. Zaiser and P. Moretti, J. Stat. Mech. P08004 (2005).[77] G. Picard, A. Ajdari, F. Lequeux, et al., Euro. Phys. J. E 15 371 (2004).[78] M. Zaiser and E.C. Aifantis, Int. J. Plasticity, in press.[79] I. Groma, F. Csikor and M. Zaiser, Acta mater. 51 1271 (2003).[80] J.-C. Baret, D. Vandembroucq and S. Roux, Phys. Rev. Lett. 89 195506 (2002).[81] V.V. Bulatov and A.A. Argon, Model. Simul. Mater. Sci. Engng. 2 167 (1994).[82] G. Picard, A. Ajdari, F. Lequeux, et al., Phys. Rev. E 71 010501 (2005).[83] M. Koslowski, A.M. Cuitino and M. Ortiz, J. Mech. Phys. Solids. 50 2597 (2002).[84] M. Koslowski, R. LeSar and R. Thomson, Phys. Rev. Lett. 93 125502 (2004).[85] Y.U. Wang, Y.M. Jin, A.M. Cuitin and A.G. Khachaturyan, Acta mater. 49 1847 (2001).[86] R.A. White and K.A. Dahmen, Phys. Rev. Lett. 91 085702 (2003).[87] K. Chen, P. Bak and S.P. Obukhov, Phys. Rev. A 42 625 (1991).[88] A. Middleton, Phys. Rev. Lett. 68 670 (1992).

Scale invariance in plastic flow of crystalline solids 245

Downloaded By: [Karlsruher Inst fur Technologie Kit] At: 14:00 9 December 2010